# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2015

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 1421262'
_audit_update_record             
;
2015-08-31 deposited with the CCDC.
2015-10-14 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'C3 H54 Mn2 N7 O55 P V18'
_chemical_formula_weight         2126.30

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Orthorhombic
_symmetry_space_group_name_H-M   P212121

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y, z+1/2'
'x+1/2, -y+1/2, -z'
'-x, y+1/2, -z+1/2'

_cell_length_a                   12.1286(19)
_cell_length_b                   20.336(3)
_cell_length_c                   21.324(3)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_volume                     5259.5(14)
_cell_formula_units_Z            4
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    ?
_cell_measurement_theta_min      1.38
_cell_measurement_theta_max      25.99

_exptl_crystal_description       block
_exptl_crystal_colour            brown
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.06
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.685
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             4160
_exptl_absorpt_coefficient_mu    3.654
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.4501
_exptl_absorpt_correction_T_max  0.8106
_exptl_absorpt_process_details   'ABSCOR by T.Higashi    8 March, 1995'

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker APEX area-detector diffractometer'
_diffrn_measurement_method       'φ and ω scan'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            32248
_diffrn_reflns_av_R_equivalents  0.0896
_diffrn_reflns_av_sigmaI/netI    0.0805
_diffrn_reflns_limit_h_min       -14
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_k_min       -25
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_l_min       -26
_diffrn_reflns_limit_l_max       26
_diffrn_reflns_theta_min         1.38
_diffrn_reflns_theta_max         25.99
_reflns_number_total             10260
_reflns_number_gt                8798
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.0974P)²+1.0883P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   none
_refine_ls_hydrogen_treatment    mixed
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.02(3)
_refine_ls_number_reflns         10260
_refine_ls_number_parameters     761
_refine_ls_number_restraints     72
_refine_ls_R_factor_all          0.0668
_refine_ls_R_factor_gt           0.0544
_refine_ls_wR_factor_ref         0.1564
_refine_ls_wR_factor_gt          0.1469
_refine_ls_goodness_of_fit_ref   1.058
_refine_ls_restrained_S_all      1.062
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
V1 V 0.64106(12) 1.01457(7) 0.46612(6) 0.0125(3) Uani 1 1 d . . .
V2 V 0.64093(12) 1.05338(8) 0.62657(7) 0.0142(3) Uani 1 1 d . . .
V3 V 0.42682(12) 1.17817(8) 0.59541(7) 0.0155(3) Uani 1 1 d . . .
V4 V 0.33391(11) 0.84116(8) 0.49445(7) 0.0116(3) Uani 1 1 d . . .
V5 V 0.13421(12) 0.96221(7) 0.46856(6) 0.0122(3) Uani 1 1 d . . .
V6 V 0.17703(12) 1.13686(8) 0.51319(7) 0.0151(3) Uani 1 1 d . . .
V7 V 0.12706(12) 1.00622(7) 0.63295(7) 0.0133(3) Uani 1 1 d . . .
V8 V 0.42770(12) 1.13910(8) 0.43198(7) 0.0145(3) Uani 1 1 d . . .
V9 V 0.38725(12) 0.96621(8) 0.38210(7) 0.0128(3) Uani 1 1 d . . .
V10 V 0.13855(12) 0.87463(7) 0.57515(7) 0.0130(3) Uani 1 1 d . . .
V11 V 0.20970(14) 1.14417(9) 0.65248(8) 0.0241(4) Uani 1 1 d . . .
V12 V 0.32393(12) 0.88268(8) 0.66220(7) 0.0135(3) Uani 1 1 d . . .
V13 V 0.54926(12) 0.94192(8) 0.69348(7) 0.0162(3) Uani 1 1 d . . .
V14 V 0.21946(12) 1.07818(8) 0.39579(7) 0.0151(3) Uani 1 1 d . . .
V15 V 0.58951(12) 0.89251(8) 0.57381(7) 0.0130(3) Uani 1 1 d . . .
V16 V 0.62902(13) 1.13762(8) 0.51990(7) 0.0182(3) Uani 1 1 d . . .
V17 V 0.37580(12) 1.05006(8) 0.70933(7) 0.0142(3) Uani 1 1 d . . .
V18 V 0.54298(12) 0.88442(8) 0.43591(7) 0.0145(3) Uani 1 1 d . . .
P1 P 0.37861(18) 1.01463(11) 0.54775(10) 0.0102(4) Uani 1 1 d . . .
Mn1 Mn 0.85875(11) 0.81933(7) 0.58645(6) 0.0170(3) Uani 1 1 d . . .
Mn2 Mn 0.70054(17) 0.93395(11) 0.83452(9) 0.0472(5) Uani 1 1 d . . .
O1 O 0.4888(5) 0.8517(3) 0.5162(3) 0.0164(13) Uani 1 1 d . . .
O2 O 0.0050(5) 1.0095(3) 0.6646(3) 0.0178(14) Uani 1 1 d . . .
O3 O 0.7291(6) 1.1897(4) 0.5061(4) 0.0347(18) Uani 1 1 d . . .
O4 O 0.4552(6) 1.2500(3) 0.6242(3) 0.0263(16) Uani 1 1 d . . .
O5 O 0.7981(9) 0.8397(6) 0.8474(6) 0.086(4) Uani 1 1 d U . .
O6 O 0.5725(6) 0.8845(4) 0.8896(4) 0.0349(18) Uani 1 1 d . . .
O7 O 0.1369(7) 1.1937(5) 0.6932(4) 0.050(2) Uani 1 1 d . . .
O8 O 0.5939(9) 1.0216(5) 0.8307(4) 0.059(3) Uani 1 1 d . . .
O9 O 0.8447(8) 0.9823(6) 0.7945(5) 0.067(3) Uani 1 1 d U . .
O10 O 0.6789(5) 0.8333(3) 0.5886(3) 0.0172(13) Uani 1 1 d . . .
O11 O 0.2872(5) 0.8441(3) 0.5825(3) 0.0142(12) Uani 1 1 d . . .
O12 O 0.4798(5) 0.8842(3) 0.6392(3) 0.0138(13) Uani 1 1 d . . .
O13 O 0.0351(5) 0.8231(3) 0.5851(3) 0.0199(14) Uani 1 1 d . . .
O14 O 0.3868(5) 0.8768(3) 0.4150(3) 0.0150(13) Uani 1 1 d . . .
O15 O 0.3731(5) 1.0637(3) 0.3869(3) 0.0144(13) Uani 1 1 d . . .
O16 O 0.1726(5) 0.9157(3) 0.6566(3) 0.0117(12) Uani 1 1 d U . .
O17 O 0.6545(4) 0.9239(3) 0.4944(3) 0.0135(13) Uani 1 1 d U . .
O18 O 0.5371(5) 0.9726(3) 0.4093(3) 0.0159(13) Uani 1 1 d . . .
O19 O 0.6573(5) 0.9586(3) 0.6304(3) 0.0178(14) Uani 1 1 d . . .
O20 O 0.1403(5) 1.0577(3) 0.4682(3) 0.0166(13) Uani 1 1 d . . .
O21 O 0.7502(5) 1.0215(3) 0.4216(3) 0.0200(14) Uani 1 1 d U . .
O22 O 0.4853(5) 1.1950(3) 0.5068(3) 0.0184(14) Uani 1 1 d . . .
O23 O 0.1803(5) 0.8717(3) 0.4849(3) 0.0124(12) Uani 1 1 d . . .
O24 O 0.3634(5) 1.1329(3) 0.6657(3) 0.0173(13) Uani 1 1 d . . .
O25 O 0.2683(5) 1.1574(3) 0.4394(3) 0.0159(13) Uani 1 1 d . . .
O26 O 0.3265(6) 0.7619(3) 0.4781(3) 0.0223(15) Uani 1 1 d . . .
O27 O 0.8533(5) 0.8813(4) 0.5024(3) 0.0264(16) Uani 1 1 d . . .
O28 O 0.3650(5) 1.0888(3) 0.5322(3) 0.0159(13) Uani 1 1 d . . .
O29 O 0.5031(5) 0.9969(3) 0.5496(3) 0.0162(13) Uani 1 1 d . . .
O30 O 0.3097(6) 0.8212(3) 0.7100(3) 0.0235(15) Uani 1 1 d . . .
O31 O 0.8552(6) 0.9028(4) 0.6513(3) 0.0312(17) Uani 1 1 d . . .
O32 O 0.3261(5) 1.0001(3) 0.6127(3) 0.0172(13) Uani 1 1 d . . .
O33 O 0.5680(5) 1.1333(3) 0.6028(3) 0.0169(13) Uani 1 1 d . . .
O34 O 0.7415(6) 1.0794(4) 0.6679(3) 0.0266(16) Uani 1 1 d . . .
O35 O 0.6156(6) 0.9081(4) 0.7524(3) 0.0285(16) Uani 1 1 d U . .
O36 O 0.2644(5) 1.1970(3) 0.5735(3) 0.0214(15) Uani 1 1 d . . .
O37 O 0.3822(6) 1.0717(4) 0.7824(3) 0.0236(15) Uani 1 1 d U . .
O38 O 0.1420(5) 1.0920(3) 0.5926(3) 0.0146(12) Uani 1 1 d U . .
O39 O 0.4010(5) 0.9542(3) 0.3073(3) 0.0212(14) Uani 1 1 d U . .
O40 O 0.0138(5) 0.9495(4) 0.4356(3) 0.0235(15) Uani 1 1 d . . .
O41 O 0.3197(5) 0.9731(3) 0.4966(3) 0.0182(14) Uani 1 1 d . . .
O42 O 0.1433(6) 1.1024(3) 0.3367(3) 0.0242(15) Uani 1 1 d . . .
O43 O 0.6088(6) 0.8369(4) 0.3865(3) 0.0321(18) Uani 1 1 d . . .
O44 O 0.6976(5) 1.0539(3) 0.5423(3) 0.0169(13) Uani 1 1 d . . .
O45 O 0.2086(5) 1.0559(3) 0.7024(3) 0.0160(13) Uani 1 1 d U . .
O46 O 0.0948(5) 0.9621(3) 0.5554(3) 0.0150(13) Uani 1 1 d U . .
O47 O 0.0704(5) 1.1837(3) 0.5029(3) 0.0215(15) Uani 1 1 d . . .
O48 O 0.5272(5) 1.0351(3) 0.6879(3) 0.0169(13) Uani 1 1 d . . .
O49 O 0.5672(5) 1.0950(3) 0.4503(3) 0.0173(14) Uani 1 1 d . . .
O50 O 0.3872(5) 0.9499(3) 0.7248(3) 0.0153(13) Uani 1 1 d . . .
O51 O 0.8517(8) 0.7384(4) 0.6565(3) 0.039(2) Uani 1 1 d . . .
O52 O 0.4626(6) 1.1895(3) 0.3770(3) 0.0253(16) Uani 1 1 d . . .
O53 O 0.2200(5) 0.9763(3) 0.3860(3) 0.0137(13) Uani 1 1 d U . .
O1W O 0.0456(8) 0.8967(5) 0.7640(4) 0.048(2) Uani 1 1 d . . .
O2W O 0.9181(7) 0.0688(6) 0.5280(5) 0.063(3) Uani 1 1 d . . .
C1 C 1.0145(12) 0.7851(7) 0.3670(6) 0.052(4) Uani 1 1 d . . .
H1A H 1.0728 0.8062 0.3432 0.062 Uiso 1 1 calc R . .
H1B H 1.0033 0.7415 0.3497 0.062 Uiso 1 1 calc R . .
C2 C 0.9087(10) 0.8247(7) 0.3603(6) 0.042(3) Uani 1 1 d . . .
H2A H 0.9188 0.8686 0.3784 0.050 Uiso 1 1 calc R . .
C3 C 0.8875(17) 0.8307(10) 0.2855(7) 0.092(7) Uani 1 1 d . . .
H3A H 0.8218 0.8559 0.2781 0.138 Uiso 1 1 calc R . .
H3B H 0.8788 0.7876 0.2679 0.138 Uiso 1 1 calc R . .
H3C H 0.9492 0.8522 0.2661 0.138 Uiso 1 1 calc R . .
N1 N 1.0496(8) 0.7792(5) 0.4355(5) 0.036(2) Uani 1 1 d . . .
H1C H 1.1109 0.7553 0.4381 0.053 Uiso 1 1 calc R . .
H1D H 0.9962 0.7598 0.4574 0.053 Uiso 1 1 calc R . .
H1E H 1.0620 0.8192 0.4511 0.053 Uiso 1 1 calc R . .
N2 N 0.8180(4) 0.7923(2) 0.3902(2) 0.031(2) Uani 1 1 d . . .
H2B H 0.8313 0.7889 0.4312 0.046 Uiso 1 1 calc R . .
H2C H 0.8096 0.7523 0.3739 0.046 Uiso 1 1 calc R . .
H2D H 0.7567 0.8155 0.3843 0.046 Uiso 1 1 calc R . .
N3 N 0.4042(4) 0.3234(2) 0.3794(2) 0.082(5) Uani 1 1 d R . .
N4 N 0.0683(4) 0.7582(2) 0.7263(2) 0.089(6) Uani 1 1 d R . .
N5 N 0.5784(4) 0.8847(2) 0.2516(2) 0.096(6) Uani 1 1 d R . .
N6 N 0.2075(4) 0.2483(2) 0.3490(2) 0.041(3) Uani 1 1 d R . .
N7 N 0.6767(4) 0.7706(2) 0.7488(2) 0.055(3) Uani 1 1 d R . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
V1 O21 1.635(6) . ?
V1 O49 1.895(6) . ?
V1 O44 1.936(6) . ?
V1 O17 1.946(6) . ?
V1 O18 1.947(6) . ?
V1 V16 2.756(2) . ?
V1 V18 2.972(2) . ?
V2 O34 1.595(7) . ?
V2 O33 1.919(6) . ?
V2 O44 1.925(6) . ?
V2 O48 1.937(6) . ?
V2 O19 1.939(7) . ?
V2 V16 2.851(2) . ?
V2 V13 2.900(2) . ?
V3 O4 1.622(7) . ?
V3 O24 1.921(6) . ?
V3 O33 1.946(6) . ?
V3 O22 2.047(7) . ?
V3 O36 2.060(6) . ?
V3 O28 2.383(6) . ?
V3 V11 2.982(2) . ?
V3 V16 3.047(2) . ?
V4 O26 1.651(7) . ?
V4 O1 1.947(6) . ?
V4 O14 1.951(6) . ?
V4 O11 1.962(6) . ?
V4 O23 1.975(6) . ?
V4 V18 2.960(2) . ?
V4 V10 3.007(2) . ?
V5 O40 1.642(6) . ?
V5 O46 1.914(6) . ?
V5 O20 1.943(6) . ?
V5 O23 1.954(6) . ?
V5 O53 2.066(6) . ?
V5 O41 2.339(6) . ?
V5 V10 2.888(2) . ?
V5 V14 3.006(2) . ?
V6 O47 1.621(6) . ?
V6 O20 1.927(6) . ?
V6 O25 1.968(6) . ?
V6 O38 1.970(6) . ?
V6 O36 2.067(7) . ?
V6 V14 2.821(2) . ?
V6 V11 3.000(2) . ?
V7 O2 1.629(6) . ?
V7 O46 1.921(6) . ?
V7 O38 1.954(6) . ?
V7 O16 1.987(6) . ?
V7 O45 2.048(6) . ?
V7 O32 2.456(6) . ?
V7 V10 2.949(2) . ?
V7 V11 3.008(2) . ?
V8 O52 1.614(6) . ?
V8 O15 1.928(6) . ?
V8 O49 1.955(6) . ?
V8 O25 1.975(6) . ?
V8 O22 2.080(7) . ?
V8 V14 2.917(2) . ?
V8 V16 3.079(2) . ?
V9 O39 1.622(6) . ?
V9 O18 1.912(6) . ?
V9 O14 1.949(6) . ?
V9 O15 1.992(6) . ?
V9 O53 2.040(6) . ?
V9 V18 2.766(2) . ?
V9 V14 3.068(2) . ?
V10 O13 1.649(7) . ?
V10 O46 1.903(6) . ?
V10 O11 1.914(6) . ?
V10 O16 1.971(6) . ?
V10 O23 1.991(6) . ?
V10 V12 2.920(2) . ?
V11 O7 1.596(8) . ?
V11 O38 1.851(6) . ?
V11 O24 1.899(6) . ?
V11 O45 2.088(7) . ?
V11 O36 2.104(7) . ?
V11 V17 3.032(2) . ?
V12 O30 1.622(7) . ?
V12 O11 1.924(6) . ?
V12 O12 1.953(6) . ?
V12 O16 1.958(6) . ?
V12 O50 2.059(6) . ?
V12 V13 3.060(2) . ?
V13 O35 1.642(7) . ?
V13 O12 1.852(6) . ?
V13 O19 1.909(6) . ?
V13 O48 1.918(7) . ?
V13 O50 2.082(6) . ?
V13 V15 2.786(2) . ?
V13 V17 3.062(2) . ?
V14 O42 1.638(6) . ?
V14 O20 1.865(6) . ?
V14 O15 1.896(6) . ?
V14 O25 1.952(7) . ?
V14 O53 2.083(6) . ?
V15 O10 1.650(6) . ?
V15 O1 1.921(6) . ?
V15 O12 1.935(6) . ?
V15 O17 1.975(6) . ?
V15 O19 1.984(6) . ?
V15 O29 2.424(7) . ?
V15 V18 2.999(2) . ?
V16 O3 1.638(8) . ?
V16 O49 1.875(6) . ?
V16 O33 1.918(6) . ?
V16 O44 1.955(7) . ?
V16 O22 2.116(7) . ?
V17 O37 1.621(6) . ?
V17 O48 1.917(6) . ?
V17 O24 1.930(7) . ?
V17 O45 2.036(6) . ?
V17 O50 2.067(6) . ?
V17 O32 2.375(6) . ?
V18 O43 1.637(7) . ?
V18 O18 1.882(6) . ?
V18 O1 1.950(6) . ?
V18 O14 1.952(6) . ?
V18 O17 2.007(6) . ?
P1 O32 1.552(6) . ?
P1 O29 1.553(6) . ?
P1 O28 1.553(6) . ?
P1 O41 1.553(7) . ?
Mn1 O13 2.140(7) 1_655 ?
Mn1 O26 2.186(7) 3_566 ?
Mn1 O31 2.191(7) . ?
Mn1 O27 2.193(7) . ?
Mn1 O10 2.201(6) . ?
Mn1 O51 2.224(8) . ?
Mn2 O35 2.099(7) . ?
Mn2 O21 2.151(6) 2_675 ?
Mn2 O9 2.180(10) . ?
Mn2 O6 2.191(8) . ?
Mn2 O8 2.203(10) . ?
Mn2 O5 2.270(11) . ?
O13 Mn1 2.140(7) 1_455 ?
O21 Mn2 2.151(6) 2_674 ?
O26 Mn1 2.186(7) 3_466 ?
C1 C2 1.522(19) . ?
C1 N1 1.528(16) . ?
C1 H1A 0.9700 . ?
C1 H1B 0.9700 . ?
C2 N2 1.433(13) . ?
C2 C3 1.620(18) . ?
C2 H2A 0.9800 . ?
C3 H3A 0.9600 . ?
C3 H3B 0.9600 . ?
C3 H3C 0.9600 . ?
N1 H1C 0.8900 . ?
N1 H1D 0.8900 . ?
N1 H1E 0.8900 . ?
N2 H2B 0.8900 . ?
N2 H2C 0.8900 . ?
N2 H2D 0.8900 . ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O21 V1 O49 101.8(3) . . ?
O21 V1 O44 99.5(3) . . ?
O49 V1 O44 87.7(3) . . ?
O21 V1 O17 101.2(3) . . ?
O49 V1 O17 155.8(3) . . ?
O44 V1 O17 95.8(3) . . ?
O21 V1 O18 101.6(3) . . ?
O49 V1 O18 87.8(3) . . ?
O44 V1 O18 159.0(3) . . ?
O17 V1 O18 80.3(2) . . ?
O21 V1 V16 101.9(2) . . ?
O49 V1 V16 42.74(19) . . ?
O44 V1 V16 45.2(2) . . ?
O17 V1 V16 137.35(18) . . ?
O18 V1 V16 128.54(19) . . ?
O21 V1 V18 105.9(2) . . ?
O49 V1 V18 122.7(2) . . ?
O44 V1 V18 133.7(2) . . ?
O17 V1 V18 42.02(17) . . ?
O18 V1 V18 38.29(18) . . ?
V16 V1 V18 151.31(7) . . ?
O34 V2 O33 102.6(3) . . ?
O34 V2 O44 103.9(3) . . ?
O33 V2 O44 85.0(3) . . ?
O34 V2 O48 103.6(3) . . ?
O33 V2 O48 90.7(3) . . ?
O44 V2 O48 152.4(3) . . ?
O34 V2 O19 103.2(3) . . ?
O33 V2 O19 154.2(3) . . ?
O44 V2 O19 90.4(3) . . ?
O48 V2 O19 81.6(3) . . ?
O34 V2 V16 106.3(3) . . ?
O33 V2 V16 41.99(18) . . ?
O44 V2 V16 43.1(2) . . ?
O48 V2 V16 128.2(2) . . ?
O19 V2 V16 129.46(19) . . ?
O34 V2 V13 106.3(3) . . ?
O33 V2 V13 128.0(2) . . ?
O44 V2 V13 126.9(2) . . ?
O48 V2 V13 40.96(19) . . ?
O19 V2 V13 40.70(19) . . ?
V16 V2 V13 147.43(7) . . ?
O4 V3 O24 102.8(3) . . ?
O4 V3 O33 101.8(3) . . ?
O24 V3 O33 93.7(3) . . ?
O4 V3 O22 97.2(3) . . ?
O24 V3 O22 160.0(3) . . ?
O33 V3 O22 81.3(3) . . ?
O4 V3 O36 97.0(3) . . ?
O24 V3 O36 83.3(3) . . ?
O33 V3 O36 161.2(3) . . ?
O22 V3 O36 95.2(3) . . ?
O4 V3 O28 165.4(3) . . ?
O24 V3 O28 87.1(2) . . ?
O33 V3 O28 88.0(2) . . ?
O22 V3 O28 73.4(2) . . ?
O36 V3 O28 73.3(2) . . ?
O4 V3 V11 104.0(3) . . ?
O24 V3 V11 38.42(19) . . ?
O33 V3 V11 129.4(2) . . ?
O22 V3 V11 136.18(19) . . ?
O36 V3 V11 44.9(2) . . ?
O28 V3 V11 77.07(16) . . ?
O4 V3 V16 105.8(3) . . ?
O24 V3 V16 127.2(2) . . ?
O33 V3 V16 37.61(18) . . ?
O22 V3 V16 43.84(18) . . ?
O36 V3 V16 134.4(2) . . ?
O28 V3 V16 75.40(16) . . ?
V11 V3 V16 149.71(7) . . ?
O26 V4 O1 102.1(3) . . ?
O26 V4 O14 101.4(3) . . ?
O1 V4 O14 81.3(3) . . ?
O26 V4 O11 102.5(3) . . ?
O1 V4 O11 92.7(3) . . ?
O14 V4 O11 156.1(3) . . ?
O26 V4 O23 103.6(3) . . ?
O1 V4 O23 154.2(3) . . ?
O14 V4 O23 96.0(2) . . ?
O11 V4 O23 79.4(2) . . ?
O26 V4 V18 104.3(2) . . ?
O1 V4 V18 40.61(18) . . ?
O14 V4 V18 40.68(18) . . ?
O11 V4 V18 129.93(19) . . ?
O23 V4 V18 132.16(19) . . ?
O26 V4 V10 107.4(2) . . ?
O1 V4 V10 126.85(19) . . ?
O14 V4 V10 132.22(19) . . ?
O11 V4 V10 38.55(17) . . ?
O23 V4 V10 40.90(17) . . ?
V18 V4 V10 148.12(7) . . ?
O40 V5 O46 101.1(3) . . ?
O40 V5 O20 100.9(3) . . ?
O46 V5 O20 90.8(3) . . ?
O40 V5 O23 100.5(3) . . ?
O46 V5 O23 84.1(3) . . ?
O20 V5 O23 158.5(3) . . ?
O40 V5 O53 96.0(3) . . ?
O46 V5 O53 162.1(3) . . ?
O20 V5 O53 80.8(2) . . ?
O23 V5 O53 97.9(2) . . ?
O40 V5 O41 168.7(3) . . ?
O46 V5 O41 89.6(2) . . ?
O20 V5 O41 82.5(3) . . ?
O23 V5 O41 76.6(2) . . ?
O53 V5 O41 73.8(2) . . ?
O40 V5 V10 104.9(3) . . ?
O46 V5 V10 40.70(19) . . ?
O20 V5 V10 128.22(19) . . ?
O23 V5 V10 43.43(17) . . ?
O53 V5 V10 138.34(18) . . ?
O41 V5 V10 80.75(16) . . ?
O40 V5 V14 102.0(3) . . ?
O46 V5 V14 125.9(2) . . ?
O20 V5 V14 36.96(18) . . ?
O23 V5 V14 137.07(18) . . ?
O53 V5 V14 43.80(17) . . ?
O41 V5 V14 74.17(16) . . ?
V10 V5 V14 152.09(7) . . ?
O47 V6 O20 103.9(3) . . ?
O47 V6 O25 102.5(3) . . ?
O20 V6 O25 84.8(3) . . ?
O47 V6 O38 102.5(3) . . ?
O20 V6 O38 89.5(3) . . ?
O25 V6 O38 155.0(3) . . ?
O47 V6 O36 98.3(3) . . ?
O20 V6 O36 157.3(3) . . ?
O25 V6 O36 94.8(3) . . ?
O38 V6 O36 81.3(3) . . ?
O47 V6 V14 105.9(3) . . ?
O20 V6 V14 41.11(18) . . ?
O25 V6 V14 43.76(19) . . ?
O38 V6 V14 127.36(19) . . ?
O36 V6 V14 135.2(2) . . ?
O47 V6 V11 102.1(3) . . ?
O20 V6 V11 124.4(2) . . ?
O25 V6 V11 134.94(19) . . ?
O38 V6 V11 36.88(17) . . ?
O36 V6 V11 44.5(2) . . ?
V14 V6 V11 151.11(8) . . ?
O2 V7 O46 101.0(3) . . ?
O2 V7 O38 103.3(3) . . ?
O46 V7 O38 93.3(3) . . ?
O2 V7 O16 100.7(3) . . ?
O46 V7 O16 80.9(3) . . ?
O38 V7 O16 156.0(3) . . ?
O2 V7 O45 96.9(3) . . ?
O46 V7 O45 162.1(3) . . ?
O38 V7 O45 80.4(3) . . ?
O16 V7 O45 98.0(3) . . ?
O2 V7 O32 165.7(3) . . ?
O46 V7 O32 91.5(2) . . ?
O38 V7 O32 82.9(2) . . ?
O16 V7 O32 74.0(2) . . ?
O45 V7 O32 71.2(2) . . ?
O2 V7 V10 104.7(2) . . ?
O46 V7 V10 39.32(19) . . ?
O38 V7 V10 128.48(18) . . ?
O16 V7 V10 41.63(17) . . ?
O45 V7 V10 136.62(19) . . ?
O32 V7 V10 80.45(16) . . ?
O2 V7 V11 102.0(2) . . ?
O46 V7 V11 128.51(19) . . ?
O38 V7 V11 36.58(17) . . ?
O16 V7 V11 137.40(18) . . ?
O45 V7 V11 43.87(18) . . ?
O32 V7 V11 75.17(16) . . ?
V10 V7 V11 152.66(7) . . ?
O52 V8 O15 103.4(3) . . ?
O52 V8 O49 102.1(3) . . ?
O15 V8 O49 91.8(3) . . ?
O52 V8 O25 101.3(3) . . ?
O15 V8 O25 81.6(3) . . ?
O49 V8 O25 156.6(3) . . ?
O52 V8 O22 97.0(3) . . ?
O15 V8 O22 158.9(3) . . ?
O49 V8 O22 78.9(3) . . ?
O25 V8 O22 99.5(3) . . ?
O52 V8 V14 107.7(3) . . ?
O15 V8 V14 39.88(18) . . ?
O49 V8 V14 127.4(2) . . ?
O25 V8 V14 41.73(19) . . ?
O22 V8 V14 136.55(18) . . ?
O52 V8 V16 103.9(3) . . ?
O15 V8 V16 124.65(19) . . ?
O49 V8 V16 35.63(19) . . ?
O25 V8 V16 136.82(19) . . ?
O22 V8 V16 43.26(18) . . ?
V14 V8 V16 147.52(7) . . ?
O39 V9 O18 102.1(3) . . ?
O39 V9 O14 102.3(3) . . ?
O18 V9 O14 87.5(3) . . ?
O39 V9 O15 102.1(3) . . ?
O18 V9 O15 90.0(3) . . ?
O14 V9 O15 155.5(2) . . ?
O39 V9 O53 99.0(3) . . ?
O18 V9 O53 157.8(3) . . ?
O14 V9 O53 94.4(3) . . ?
O15 V9 O53 79.2(3) . . ?
O39 V9 V18 104.3(3) . . ?
O18 V9 V18 42.77(18) . . ?
O14 V9 V18 44.88(18) . . ?
O15 V9 V18 129.51(18) . . ?
O53 V9 V18 136.25(18) . . ?
O39 V9 V14 105.9(2) . . ?
O18 V9 V14 123.5(2) . . ?
O14 V9 V14 131.03(18) . . ?
O15 V9 V14 36.82(18) . . ?
O53 V9 V14 42.47(18) . . ?
V18 V9 V14 149.30(7) . . ?
O13 V10 O46 114.2(3) . . ?
O13 V10 O11 120.0(3) . . ?
O46 V10 O11 125.8(3) . . ?
O13 V10 O16 108.4(3) . . ?
O46 V10 O16 81.8(3) . . ?
O11 V10 O16 82.4(2) . . ?
O13 V10 O23 107.4(3) . . ?
O46 V10 O23 83.4(3) . . ?
O11 V10 O23 80.2(2) . . ?
O16 V10 O23 144.2(3) . . ?
O13 V10 V5 118.7(2) . . ?
O46 V10 V5 40.96(18) . . ?
O11 V10 V5 106.38(19) . . ?
O16 V10 V5 115.86(19) . . ?
O23 V10 V5 42.44(18) . . ?
O13 V10 V12 122.7(2) . . ?
O46 V10 V12 107.63(19) . . ?
O11 V10 V12 40.58(18) . . ?
O16 V10 V12 41.81(17) . . ?
O23 V10 V12 114.85(18) . . ?
V5 V10 V12 118.67(7) . . ?
O13 V10 V7 119.1(2) . . ?
O46 V10 V7 39.75(18) . . ?
O11 V10 V7 107.8(2) . . ?
O16 V10 V7 42.04(18) . . ?
O23 V10 V7 116.28(19) . . ?
V5 V10 V7 76.62(6) . . ?
V12 V10 V7 73.74(5) . . ?
O13 V10 V4 122.0(2) . . ?
O46 V10 V4 107.76(19) . . ?
O11 V10 V4 39.73(17) . . ?
O16 V10 V4 115.79(17) . . ?
O23 V10 V4 40.49(17) . . ?
V5 V10 V4 72.75(5) . . ?
V12 V10 V4 76.69(5) . . ?
V7 V10 V4 118.81(6) . . ?
O7 V11 O38 119.4(4) . . ?
O7 V11 O24 122.6(4) . . ?
O38 V11 O24 117.9(3) . . ?
O7 V11 O45 105.2(4) . . ?
O38 V11 O45 81.8(3) . . ?
O24 V11 O45 80.0(3) . . ?
O7 V11 O36 106.7(4) . . ?
O38 V11 O36 83.1(3) . . ?
O24 V11 O36 82.6(3) . . ?
O45 V11 O36 148.1(3) . . ?
O7 V11 V3 124.4(4) . . ?
O38 V11 V3 104.1(2) . . ?
O24 V11 V3 38.93(19) . . ?
O45 V11 V3 114.39(17) . . ?
O36 V11 V3 43.68(17) . . ?
O7 V11 V6 119.8(4) . . ?
O38 V11 V6 39.69(19) . . ?
O24 V11 V6 105.71(19) . . ?
O45 V11 V6 117.50(18) . . ?
O36 V11 V6 43.52(18) . . ?
V3 V11 V6 73.98(6) . . ?
O7 V11 V7 118.6(4) . . ?
O38 V11 V7 38.99(19) . . ?
O24 V11 V7 103.6(2) . . ?
O45 V11 V7 42.82(17) . . ?
O36 V11 V7 118.05(19) . . ?
V3 V11 V7 116.99(7) . . ?
V6 V11 V7 76.86(6) . . ?
O7 V11 V17 123.3(4) . . ?
O38 V11 V17 102.1(2) . . ?
O24 V11 V17 38.0(2) . . ?
O45 V11 V17 42.02(16) . . ?
O36 V11 V17 115.63(19) . . ?
V3 V11 V17 73.90(6) . . ?
V6 V11 V17 116.90(7) . . ?
V7 V11 V17 71.82(6) . . ?
O30 V12 O11 102.4(3) . . ?
O30 V12 O12 105.8(3) . . ?
O11 V12 O12 90.5(2) . . ?
O30 V12 O16 101.7(3) . . ?
O11 V12 O16 82.5(2) . . ?
O12 V12 O16 152.4(3) . . ?
O30 V12 O50 98.3(3) . . ?
O11 V12 O50 158.4(3) . . ?
O12 V12 O50 78.0(3) . . ?
O16 V12 O50 99.2(2) . . ?
O30 V12 V10 105.9(2) . . ?
O11 V12 V10 40.32(18) . . ?
O12 V12 V10 125.89(18) . . ?
O16 V12 V10 42.16(17) . . ?
O50 V12 V10 137.38(19) . . ?
O30 V12 V13 105.2(2) . . ?
O11 V12 V13 124.05(19) . . ?
O12 V12 V13 35.34(18) . . ?
O16 V12 V13 135.67(19) . . ?
O50 V12 V13 42.66(18) . . ?
V10 V12 V13 148.01(7) . . ?
O35 V13 O12 115.8(3) . . ?
O35 V13 O19 106.1(3) . . ?
O12 V13 O19 89.1(3) . . ?
O35 V13 O48 122.0(3) . . ?
O12 V13 O48 121.6(3) . . ?
O19 V13 O48 82.9(3) . . ?
O35 V13 O50 104.5(3) . . ?
O12 V13 O50 79.6(3) . . ?
O19 V13 O50 149.3(3) . . ?
O48 V13 O50 79.1(3) . . ?
O35 V13 V15 117.6(3) . . ?
O12 V13 V15 43.80(18) . . ?
O19 V13 V15 45.41(18) . . ?
O48 V13 V15 108.9(2) . . ?
O50 V13 V15 119.15(17) . . ?
O35 V13 V2 121.0(3) . . ?
O12 V13 V2 111.2(2) . . ?
O19 V13 V2 41.5(2) . . ?
O48 V13 V2 41.45(19) . . ?
O50 V13 V2 117.27(19) . . ?
V15 V13 V2 76.35(6) . . ?
O35 V13 V12 116.1(3) . . ?
O12 V13 V12 37.59(18) . . ?
O19 V13 V12 121.96(18) . . ?
O48 V13 V12 104.6(2) . . ?
O50 V13 V12 42.06(17) . . ?
V15 V13 V12 79.33(6) . . ?
V2 V13 V12 122.88(6) . . ?
O35 V13 V17 123.6(3) . . ?
O12 V13 V17 102.2(2) . . ?
O19 V13 V17 114.9(2) . . ?
O48 V13 V17 37.00(19) . . ?
O50 V13 V17 42.24(18) . . ?
V15 V13 V17 118.72(6) . . ?
V2 V13 V17 75.90(6) . . ?
V12 V13 V17 72.13(5) . . ?
O42 V14 O20 114.4(3) . . ?
O42 V14 O15 121.6(3) . . ?
O20 V14 O15 123.6(3) . . ?
O42 V14 O25 106.8(3) . . ?
O20 V14 O25 86.9(3) . . ?
O15 V14 O25 83.0(3) . . ?
O42 V14 O53 102.9(3) . . ?
O20 V14 O53 82.1(3) . . ?
O15 V14 O53 80.3(3) . . ?
O25 V14 O53 150.2(3) . . ?
O42 V14 V6 116.9(3) . . ?
O20 V14 V6 42.78(19) . . ?
O15 V14 V6 109.53(19) . . ?
O25 V14 V6 44.22(18) . . ?
O53 V14 V6 120.72(17) . . ?
O42 V14 V8 124.3(3) . . ?
O20 V14 V8 108.8(2) . . ?
O15 V14 V8 40.70(19) . . ?
O25 V14 V8 42.33(18) . . ?
O53 V14 V8 116.51(18) . . ?
V6 V14 V8 75.14(6) . . ?
O42 V14 V5 116.0(3) . . ?
O20 V14 V5 38.77(19) . . ?
O15 V14 V5 105.53(19) . . ?
O25 V14 V5 120.37(19) . . ?
O53 V14 V5 43.33(16) . . ?
V6 V14 V5 79.11(6) . . ?
V8 V14 V5 119.63(6) . . ?
O42 V14 V9 121.6(3) . . ?
O20 V14 V9 104.7(2) . . ?
O15 V14 V9 39.02(19) . . ?
O25 V14 V9 117.15(18) . . ?
O53 V14 V9 41.39(17) . . ?
V6 V14 V9 121.30(6) . . ?
V8 V14 V9 76.47(5) . . ?
V5 V14 V9 72.24(5) . . ?
O10 V15 O1 103.0(3) . . ?
O10 V15 O12 104.5(3) . . ?
O1 V15 O12 89.2(3) . . ?
O10 V15 O17 97.9(3) . . ?
O1 V15 O17 81.1(2) . . ?
O12 V15 O17 157.1(3) . . ?
O10 V15 O19 96.1(3) . . ?
O1 V15 O19 160.9(3) . . ?
O12 V15 O19 84.6(3) . . ?
O17 V15 O19 97.9(3) . . ?
O10 V15 O29 164.5(3) . . ?
O1 V15 O29 88.1(2) . . ?
O12 V15 O29 86.1(2) . . ?
O17 V15 O29 72.9(2) . . ?
O19 V15 O29 73.4(2) . . ?
O10 V15 V13 101.7(2) . . ?
O1 V15 V13 129.11(19) . . ?
O12 V15 V13 41.49(18) . . ?
O17 V15 V13 137.65(19) . . ?
O19 V15 V13 43.23(19) . . ?
O29 V15 V13 78.64(15) . . ?
O10 V15 V18 105.7(2) . . ?
O1 V15 V18 39.57(18) . . ?
O12 V15 V18 124.90(18) . . ?
O17 V15 V18 41.55(17) . . ?
O19 V15 V18 135.3(2) . . ?
O29 V15 V18 76.00(15) . . ?
V13 V15 V18 152.26(7) . . ?
O3 V16 O49 116.9(4) . . ?
O3 V16 O33 118.8(4) . . ?
O49 V16 O33 123.6(3) . . ?
O3 V16 O44 107.0(3) . . ?
O49 V16 O44 87.7(3) . . ?
O33 V16 O44 84.2(3) . . ?
O3 V16 O22 103.3(3) . . ?
O49 V16 O22 79.7(3) . . ?
O33 V16 O22 80.1(3) . . ?
O44 V16 O22 149.7(3) . . ?
O3 V16 V1 118.2(3) . . ?
O49 V16 V1 43.3(2) . . ?
O33 V16 V1 111.3(2) . . ?
O44 V16 V1 44.61(18) . . ?
O22 V16 V1 119.31(19) . . ?
O3 V16 V2 119.7(3) . . ?
O49 V16 V2 112.0(2) . . ?
O33 V16 V2 42.02(19) . . ?
O44 V16 V2 42.28(18) . . ?
O22 V16 V2 118.57(19) . . ?
V1 V16 V2 77.52(6) . . ?
O3 V16 V3 121.1(3) . . ?
O49 V16 V3 102.8(2) . . ?
O33 V16 V3 38.27(19) . . ?
O44 V16 V3 116.70(19) . . ?
O22 V16 V3 42.06(18) . . ?
V1 V16 V3 120.54(7) . . ?
V2 V16 V3 77.40(6) . . ?
O3 V16 V8 118.1(3) . . ?
O49 V16 V8 37.39(19) . . ?
O33 V16 V8 104.8(2) . . ?
O44 V16 V8 119.66(19) . . ?
O22 V16 V8 42.36(18) . . ?
V1 V16 V8 78.32(6) . . ?
V2 V16 V8 122.14(7) . . ?
V3 V16 V8 71.39(5) . . ?
O37 V17 O48 103.1(3) . . ?
O37 V17 O24 103.3(3) . . ?
O48 V17 O24 95.6(3) . . ?
O37 V17 O45 95.8(3) . . ?
O48 V17 O45 161.1(3) . . ?
O24 V17 O45 80.6(3) . . ?
O37 V17 O50 96.4(3) . . ?
O48 V17 O50 79.5(3) . . ?
O24 V17 O50 160.3(3) . . ?
O45 V17 O50 97.8(3) . . ?
O37 V17 O32 164.2(3) . . ?
O48 V17 O32 88.2(2) . . ?
O24 V17 O32 86.3(2) . . ?
O45 V17 O32 73.1(2) . . ?
O50 V17 O32 74.6(2) . . ?
O37 V17 V11 104.2(3) . . ?
O48 V17 V11 129.9(2) . . ?
O24 V17 V11 37.30(19) . . ?
O45 V17 V11 43.35(19) . . ?
O50 V17 V11 136.87(19) . . ?
O32 V17 V11 75.79(16) . . ?
O37 V17 V13 105.5(3) . . ?
O48 V17 V13 37.0(2) . . ?
O24 V17 V13 128.8(2) . . ?
O45 V17 V13 135.87(19) . . ?
O50 V17 V13 42.64(18) . . ?
O32 V17 V13 76.78(16) . . ?
V11 V17 V13 149.97(7) . . ?
O43 V18 O18 112.7(3) . . ?
O43 V18 O1 121.8(3) . . ?
O18 V18 O1 125.3(3) . . ?
O43 V18 O14 106.2(3) . . ?
O18 V18 O14 88.3(3) . . ?
O1 V18 O14 81.2(3) . . ?
O43 V18 O17 107.9(3) . . ?
O18 V18 O17 80.3(3) . . ?
O1 V18 O17 79.6(2) . . ?
O14 V18 O17 145.8(3) . . ?
O43 V18 V9 114.9(3) . . ?
O18 V18 V9 43.61(19) . . ?
O1 V18 V9 109.84(19) . . ?
O14 V18 V9 44.79(18) . . ?
O17 V18 V9 118.49(19) . . ?
O43 V18 V4 120.9(3) . . ?
O18 V18 V4 112.2(2) . . ?
O1 V18 V4 40.54(18) . . ?
O14 V18 V4 40.67(18) . . ?
O17 V18 V4 115.75(17) . . ?
V9 V18 V4 76.63(6) . . ?
O43 V18 V1 118.0(3) . . ?
O18 V18 V1 39.87(19) . . ?
O1 V18 V1 104.40(19) . . ?
O14 V18 V1 120.56(19) . . ?
O17 V18 V1 40.47(17) . . ?
V9 V18 V1 80.08(6) . . ?
V4 V18 V1 121.07(6) . . ?
O43 V18 V15 124.9(3) . . ?
O18 V18 V15 104.5(2) . . ?
O1 V18 V15 38.88(18) . . ?
O14 V18 V15 114.27(18) . . ?
O17 V18 V15 40.74(16) . . ?
V9 V18 V15 120.15(7) . . ?
V4 V18 V15 76.35(5) . . ?
V1 V18 V15 70.33(5) . . ?
O32 P1 O29 109.4(4) . . ?
O32 P1 O28 109.4(4) . . ?
O29 P1 O28 109.5(4) . . ?
O32 P1 O41 109.5(3) . . ?
O29 P1 O41 109.8(4) . . ?
O28 P1 O41 109.3(4) . . ?
O13 Mn1 O26 101.4(3) 1_655 3_566 ?
O13 Mn1 O31 90.0(3) 1_655 . ?
O26 Mn1 O31 168.6(3) 3_566 . ?
O13 Mn1 O27 89.9(3) 1_655 . ?
O26 Mn1 O27 85.1(3) 3_566 . ?
O31 Mn1 O27 94.0(3) . . ?
O13 Mn1 O10 170.5(2) 1_655 . ?
O26 Mn1 O10 86.2(2) 3_566 . ?
O31 Mn1 O10 82.4(3) . . ?
O27 Mn1 O10 85.0(2) . . ?
O13 Mn1 O51 94.2(3) 1_655 . ?
O26 Mn1 O51 81.8(3) 3_566 . ?
O31 Mn1 O51 98.6(3) . . ?
O27 Mn1 O51 166.7(3) . . ?
O10 Mn1 O51 92.5(3) . . ?
O35 Mn2 O21 164.2(3) . 2_675 ?
O35 Mn2 O9 100.4(4) . . ?
O21 Mn2 O9 85.7(4) 2_675 . ?
O35 Mn2 O6 89.1(3) . . ?
O21 Mn2 O6 85.8(3) 2_675 . ?
O9 Mn2 O6 170.1(4) . . ?
O35 Mn2 O8 83.3(3) . . ?
O21 Mn2 O8 81.6(3) 2_675 . ?
O9 Mn2 O8 95.3(4) . . ?
O6 Mn2 O8 88.6(4) . . ?
O35 Mn2 O5 98.3(4) . . ?
O21 Mn2 O5 96.1(4) 2_675 . ?
O9 Mn2 O5 90.5(5) . . ?
O6 Mn2 O5 85.2(4) . . ?
O8 Mn2 O5 173.6(5) . . ?
V15 O1 V4 144.4(3) . . ?
V15 O1 V18 101.5(3) . . ?
V4 O1 V18 98.9(3) . . ?
V15 O10 Mn1 137.9(4) . . ?
V10 O11 V12 99.1(3) . . ?
V10 O11 V4 101.7(3) . . ?
V12 O11 V4 142.2(3) . . ?
V13 O12 V15 94.7(3) . . ?
V13 O12 V12 107.1(3) . . ?
V15 O12 V12 148.0(3) . . ?
V10 O13 Mn1 141.7(4) . 1_455 ?
V9 O14 V4 131.3(3) . . ?
V9 O14 V18 90.3(3) . . ?
V4 O14 V18 98.6(3) . . ?
V14 O15 V8 99.4(3) . . ?
V14 O15 V9 104.2(3) . . ?
V8 O15 V9 141.9(3) . . ?
V12 O16 V10 96.0(2) . . ?
V12 O16 V7 126.4(3) . . ?
V10 O16 V7 96.3(3) . . ?
V1 O17 V15 122.6(3) . . ?
V1 O17 V18 97.5(2) . . ?
V15 O17 V18 97.7(3) . . ?
V18 O18 V9 93.6(3) . . ?
V18 O18 V1 101.8(3) . . ?
V9 O18 V1 146.5(4) . . ?
V13 O19 V2 97.8(3) . . ?
V13 O19 V15 91.4(3) . . ?
V2 O19 V15 127.3(3) . . ?
V14 O20 V6 96.1(3) . . ?
V14 O20 V5 104.3(3) . . ?
V6 O20 V5 147.4(4) . . ?
V1 O21 Mn2 139.7(4) . 2_674 ?
V3 O22 V8 120.0(3) . . ?
V3 O22 V16 94.1(3) . . ?
V8 O22 V16 94.4(3) . . ?
V5 O23 V4 125.8(3) . . ?
V5 O23 V10 94.1(2) . . ?
V4 O23 V10 98.6(3) . . ?
V11 O24 V3 102.7(3) . . ?
V11 O24 V17 104.7(3) . . ?
V3 O24 V17 139.8(4) . . ?
V14 O25 V6 92.0(3) . . ?
V14 O25 V8 95.9(3) . . ?
V6 O25 V8 125.1(3) . . ?
V4 O26 Mn1 149.4(4) . 3_466 ?
P1 O28 V3 125.9(3) . . ?
P1 O29 V15 129.0(4) . . ?
P1 O32 V17 126.0(4) . . ?
P1 O32 V7 123.4(3) . . ?
V17 O32 V7 94.3(2) . . ?
V16 O33 V2 96.0(3) . . ?
V16 O33 V3 104.1(3) . . ?
V2 O33 V3 145.5(4) . . ?
V13 O35 Mn2 140.7(5) . . ?
V3 O36 V6 121.4(3) . . ?
V3 O36 V11 91.5(3) . . ?
V6 O36 V11 92.0(3) . . ?
V11 O38 V7 104.4(3) . . ?
V11 O38 V6 103.4(3) . . ?
V7 O38 V6 144.2(3) . . ?
P1 O41 V5 132.3(4) . . ?
V2 O44 V1 130.9(3) . . ?
V2 O44 V16 94.6(3) . . ?
V1 O44 V16 90.2(3) . . ?
V17 O45 V7 120.3(3) . . ?
V17 O45 V11 94.6(3) . . ?
V7 O45 V11 93.3(3) . . ?
V10 O46 V5 98.3(3) . . ?
V10 O46 V7 100.9(3) . . ?
V5 O46 V7 141.4(4) . . ?
V13 O48 V17 106.0(3) . . ?
V13 O48 V2 97.6(3) . . ?
V17 O48 V2 144.4(4) . . ?
V16 O49 V1 94.0(3) . . ?
V16 O49 V8 107.0(3) . . ?
V1 O49 V8 147.2(4) . . ?
V12 O50 V17 121.8(3) . . ?
V12 O50 V13 95.3(2) . . ?
V17 O50 V13 95.1(3) . . ?
V9 O53 V5 121.4(3) . . ?
V9 O53 V14 96.1(3) . . ?
V5 O53 V14 92.9(2) . . ?
C2 C1 N1 111.4(11) . . ?
C2 C1 H1A 109.3 . . ?
N1 C1 H1A 109.3 . . ?
C2 C1 H1B 109.3 . . ?
N1 C1 H1B 109.3 . . ?
H1A C1 H1B 108.0 . . ?
N2 C2 C1 111.2(10) . . ?
N2 C2 C3 110.6(10) . . ?
C1 C2 C3 105.4(13) . . ?
N2 C2 H2A 109.9 . . ?
C1 C2 H2A 109.9 . . ?
C3 C2 H2A 109.9 . . ?
C2 C3 H3A 109.5 . . ?
C2 C3 H3B 109.5 . . ?
H3A C3 H3B 109.5 . . ?
C2 C3 H3C 109.5 . . ?
H3A C3 H3C 109.5 . . ?
H3B C3 H3C 109.5 . . ?
C1 N1 H1C 109.5 . . ?
C1 N1 H1D 109.5 . . ?
H1C N1 H1D 109.5 . . ?
C1 N1 H1E 109.5 . . ?
H1C N1 H1E 109.5 . . ?
H1D N1 H1E 109.5 . . ?
C2 N2 H2B 109.5 . . ?
C2 N2 H2C 109.5 . . ?
H2B N2 H2C 109.5 . . ?
C2 N2 H2D 109.5 . . ?
H2B N2 H2D 109.5 . . ?
H2C N2 H2D 109.5 . . ?

_diffrn_measured_fraction_theta_max 0.996
_diffrn_reflns_theta_full        25.99
_diffrn_measured_fraction_theta_full 0.996
_refine_diff_density_max         1.373
_refine_diff_density_min         -1.832
_refine_diff_density_rms         0.229
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 1428572'
_audit_update_record             
;
2015-09-29 deposited with the CCDC.
2015-10-14 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-97
_chemical_name_systematic        
; 
 ? 
;
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'H37 Mn4 O61 P V18'
_chemical_formula_weight         2180.95

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mn Mn 0.3368 0.7283 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_symmetry_cell_setting           Tetragonal
_symmetry_space_group_name_H-M   I41/acd

loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y+1/4, x+3/4, z+1/4'
'-x+1/2, -y, z+1/2'
'y+1/4, -x+1/4, z+3/4'
'x, -y, -z+1/2'
'y+1/4, x+3/4, -z+3/4'
'-x+1/2, y, -z'
'-y+1/4, -x+1/4, -z+1/4'
'x+1/2, y+1/2, z+1/2'
'-y+3/4, x+5/4, z+3/4'
'-x+1, -y+1/2, z+1'
'y+3/4, -x+3/4, z+5/4'
'x+1/2, -y+1/2, -z+1'
'y+3/4, x+5/4, -z+5/4'
'-x+1, y+1/2, -z+1/2'
'-y+3/4, -x+3/4, -z+3/4'
'-x, -y, -z'
'y-1/4, -x-3/4, -z-1/4'
'x-1/2, y, -z-1/2'
'-y-1/4, x-1/4, -z-3/4'
'-x, y, z-1/2'
'-y-1/4, -x-3/4, z-3/4'
'x-1/2, -y, z'
'y-1/4, x-1/4, z-1/4'
'-x+1/2, -y+1/2, -z+1/2'
'y+1/4, -x-1/4, -z+1/4'
'x, y+1/2, -z'
'-y+1/4, x+1/4, -z-1/4'
'-x+1/2, y+1/2, z'
'-y+1/4, -x-1/4, z-1/4'
'x, -y+1/2, z+1/2'
'y+1/4, x+1/4, z+1/4'

_cell_length_a                   29.0398(13)
_cell_length_b                   29.0398(13)
_cell_length_c                   24.4712(19)
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_volume                     20637(2)
_cell_formula_units_Z            16
_cell_measurement_temperature    293(2)
_cell_measurement_reflns_used    ?
_cell_measurement_theta_min      1.40
_cell_measurement_theta_max      25.08

_exptl_crystal_description       block
_exptl_crystal_colour            brown
_exptl_crystal_size_max          0.26
_exptl_crystal_size_mid          0.12
_exptl_crystal_size_min          0.08
_exptl_crystal_density_meas      ?
_exptl_crystal_density_diffrn    2.808
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             16864
_exptl_absorpt_coefficient_mu    4.194
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  0.4085
_exptl_absorpt_correction_T_max  0.7302
_exptl_absorpt_process_details   'ABSCOR by T.Higashi    8 March, 1995'

_exptl_special_details           
; 
 ? 
;

_diffrn_ambient_temperature      293(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_monochromator  graphite
_diffrn_measurement_device_type  'Bruker APEX area-detector diffractometer'
_diffrn_measurement_method       'φ and ω scan'
_diffrn_detector_area_resol_mean ?
_diffrn_standards_number         ?
_diffrn_standards_interval_count ?
_diffrn_standards_interval_time  ?
_diffrn_standards_decay_%        ?
_diffrn_reflns_number            57325
_diffrn_reflns_av_R_equivalents  0.1047
_diffrn_reflns_av_sigmaI/netI    0.0413
_diffrn_reflns_limit_h_min       -34
_diffrn_reflns_limit_h_max       34
_diffrn_reflns_limit_k_min       -27
_diffrn_reflns_limit_k_max       34
_diffrn_reflns_limit_l_min       -29
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_theta_min         1.40
_diffrn_reflns_theta_max         25.08
_reflns_number_total             4594
_reflns_number_gt                3103
_reflns_threshold_expression     >2sigma(I)

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_molecular_graphics    ?
_computing_publication_material  ?

_refine_special_details          
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
;

_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'calc w=1/[σ²(Fo²)+(0.2000P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_atom_sites_solution_hydrogens   none
_refine_ls_hydrogen_treatment    none
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       ?
_refine_ls_number_reflns         4594
_refine_ls_number_parameters     403
_refine_ls_number_restraints     36
_refine_ls_R_factor_all          0.0962
_refine_ls_R_factor_gt           0.0626
_refine_ls_wR_factor_ref         0.2562
_refine_ls_wR_factor_gt          0.2128
_refine_ls_goodness_of_fit_ref   0.983
_refine_ls_restrained_S_all      0.987
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
V1 V 0.25034(5) 0.79022(5) 0.60283(7) 0.0153(4) Uani 1 1 d . . .
V2 V 0.34083(6) 0.70239(6) 0.60234(7) 0.0187(4) Uani 1 1 d . . .
V3 V 0.16175(6) 0.79185(6) 0.50556(7) 0.0167(4) Uani 1 1 d . . .
V4 V 0.16604(5) 0.70658(5) 0.60838(6) 0.0129(4) Uani 1 1 d . . .
V5 V 0.25608(6) 0.70278(5) 0.66544(7) 0.0157(4) Uani 1 1 d . . .
V6 V 0.2500 0.84042(8) 0.5000 0.0203(6) Uani 1 2 d S . .
V7 V 0.38610(6) 0.70712(6) 0.49052(7) 0.0210(5) Uani 1 1 d . . .
V8 V 0.33666(5) 0.61551(5) 0.49689(6) 0.0159(4) Uani 1 1 d . . .
V9 V 0.24416(5) 0.61669(6) 0.39530(7) 0.0169(4) Uani 1 1 d . . .
V10 V 0.2500 0.56316(10) 0.5000 0.0356(7) Uani 1 2 d S . .
Mn1 Mn 0.19216(5) 0.80510(5) 0.70386(6) 0.0208(4) Uani 1 1 d . . .
Mn2 Mn 0.5000 0.7500 0.48783(16) 0.0645(10) Uani 1 2 d S . .
Mn3 Mn 0.20805(15) 0.95165(13) 0.54257(18) 0.0436(10) Uani 0.50 1 d PU . .
P1 P 0.2500 0.70036(11) 0.5000 0.0128(8) Uani 1 2 d S . .
O1 O 0.2500 0.8978(4) 0.5000 0.047(3) Uani 1 2 d S . .
O2 O 0.2877(2) 0.5957(2) 0.4502(3) 0.0215(15) Uani 1 1 d . . .
O3 O 0.2226(2) 0.7308(2) 0.5403(3) 0.0198(15) Uani 1 1 d . . .
O4 O 0.2843(2) 0.6691(2) 0.5319(3) 0.0226(16) Uani 1 1 d . . .
O5 O 0.2483(2) 0.5769(2) 0.3486(3) 0.0247(16) Uani 1 1 d . . .
O6 O 0.2998(2) 0.5828(2) 0.5545(3) 0.0228(16) Uani 1 1 d . . .
O7 O 0.2500 0.5066(5) 0.5000 0.091(7) Uani 1 2 d S . .
O8 O 0.3772(2) 0.5770(2) 0.4865(3) 0.0271(17) Uani 1 1 d . . .
O9 O 0.2079(2) 0.7497(2) 0.6463(3) 0.0159(14) Uani 1 1 d . . .
O10 O 0.2048(2) 0.8190(2) 0.5547(3) 0.0202(15) Uani 1 1 d . . .
O11 O 0.2135(2) 0.6631(2) 0.6307(3) 0.0187(15) Uani 1 1 d . . .
O12 O 0.2511(2) 0.8301(2) 0.6510(3) 0.0246(16) Uani 1 1 d . . .
O13 O 0.2928(2) 0.8112(2) 0.5474(3) 0.0208(15) Uani 1 1 d . . .
O14 O 0.3571(2) 0.7435(2) 0.5436(3) 0.0203(15) Uani 1 1 d . . .
O15 O 0.3013(2) 0.6573(2) 0.6382(3) 0.0195(15) Uani 1 1 d . . .
O16 O 0.3727(2) 0.6575(2) 0.5494(3) 0.0210(15) Uani 1 1 d . . .
O17 O 0.1279(2) 0.6987(3) 0.6551(3) 0.0262(17) Uani 1 1 d . . .
O18 O 0.3819(3) 0.7068(3) 0.6466(3) 0.0332(19) Uani 1 1 d . . .
O19 O 0.2948(2) 0.7448(2) 0.6280(3) 0.0169(14) Uani 1 1 d . . .
O20 O 0.1358(2) 0.7532(2) 0.5627(3) 0.0205(15) Uani 1 1 d . . .
O21 O 0.2596(2) 0.7002(2) 0.7327(3) 0.0236(16) Uani 1 1 d . . .
O22 O 0.1222(3) 0.8300(3) 0.4995(3) 0.034(2) Uani 1 1 d . . .
O23 O 0.1451(2) 0.6636(2) 0.5529(3) 0.0145(14) Uani 1 1 d U . .
O24 O 0.4425(3) 0.7071(3) 0.4869(4) 0.041(2) Uani 1 1 d . A .
O25 O 0.1360(3) 0.8213(3) 0.6470(4) 0.054(3) Uani 1 1 d . . .
O26 O 0.1403(3) 0.7671(3) 0.7484(3) 0.049(2) Uani 1 1 d . . .
O27 O 0.4628(5) 0.7873(5) 0.4251(6) 0.099(4) Uani 1 1 d U A .
O28 O 0.4799(14) 0.7892(13) 0.5661(18) 0.109(13) Uani 0.40 1 d PU A 1
O28A O 0.4654(8) 0.7992(8) 0.5366(12) 0.096(8) Uiso 0.60 1 d P A 2
O29 O 0.1572(7) 0.9044(6) 0.5690(8) 0.055(5) Uani 0.50 1 d PU . .
O30 O 0.1602(6) 0.9664(9) 0.4808(10) 0.081(8) Uani 0.50 1 d P . .
O31 O 0.2394(10) 0.9286(10) 0.6238(13) 0.111(10) Uani 0.50 1 d PU . .
O1W O 0.1671(5) 0.6762(5) 0.7760(8) 0.129(7) Uani 1 1 d . . .
O2W O 0.3391(15) 0.8814(16) 0.617(3) 0.17(2) Uiso 0.40 1 d P . .
O3W O 0.3801(12) 0.8183(12) 0.6408(15) 0.169(13) Uiso 0.60 1 d P . .


_geom_special_details            
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
V1 O12 1.654(7) . ?
V1 O13 1.933(7) . ?
V1 O19 1.944(6) . ?
V1 O10 1.958(7) . ?
V1 O9 2.008(7) . ?
V1 O3 2.443(7) . ?
V1 V5 2.970(2) . ?
V2 O18 1.616(7) . ?
V2 O19 1.924(6) . ?
V2 O14 1.928(7) . ?
V2 O15 1.950(7) . ?
V2 O16 2.056(7) . ?
V2 V5 2.905(2) . ?
V2 V7 3.039(2) . ?
V3 O22 1.603(7) . ?
V3 O10 1.906(7) . ?
V3 O14 1.927(7) 7_556 ?
V3 O13 1.933(7) 7_556 ?
V3 O20 1.944(7) . ?
V3 V7 2.827(2) 7_556 ?
V3 V6 2.928(2) . ?
V4 O17 1.608(7) . ?
V4 O23 1.942(6) . ?
V4 O11 1.948(6) . ?
V4 O20 1.963(7) . ?
V4 O9 1.977(7) . ?
V4 O3 2.444(6) . ?
V4 V7 2.855(2) 7_556 ?
V4 V5 2.966(2) . ?
V5 O21 1.651(7) . ?
V5 O19 1.896(7) . ?
V5 O11 1.892(7) . ?
V5 O15 1.979(7) . ?
V5 O9 2.007(6) . ?
V5 V9 2.909(2) 7_556 ?
V6 O1 1.667(11) . ?
V6 O13 1.899(7) 7_556 ?
V6 O13 1.899(7) . ?
V6 O10 1.975(7) . ?
V6 O10 1.975(7) 7_556 ?
V6 V1 2.908(2) 7_556 ?
V6 V3 2.928(2) 7_556 ?
V7 O24 1.641(8) . ?
V7 O14 1.875(7) . ?
V7 O23 1.883(6) 7_556 ?
V7 O20 1.974(7) 7_556 ?
V7 O16 2.075(7) . ?
V7 V3 2.827(2) 7_556 ?
V7 V4 2.855(2) 7_556 ?
V7 V8 3.027(2) . ?
V8 O8 1.642(7) . ?
V8 O2 1.913(7) . ?
V8 O23 1.927(6) 7_556 ?
V8 O6 2.009(7) . ?
V8 O16 2.058(7) . ?
V8 O4 2.338(7) . ?
V8 V10 2.941(2) . ?
V9 O5 1.631(7) . ?
V9 O11 1.933(6) 7_556 ?
V9 O2 1.942(7) . ?
V9 O15 1.951(7) 7_556 ?
V9 O6 2.027(7) 7_556 ?
V9 V5 2.909(2) 7_556 ?
V9 V10 3.001(2) . ?
V10 O7 1.644(13) . ?
V10 O2 1.892(7) 7_556 ?
V10 O2 1.892(7) . ?
V10 O6 2.047(7) 7_556 ?
V10 O6 2.047(7) . ?
V10 V8 2.941(2) 7_556 ?
V10 V9 3.001(2) 7_556 ?
Mn1 O21 2.096(7) 25_566 ?
Mn1 O26 2.162(9) . ?
Mn1 O9 2.187(6) . ?
Mn1 O8 2.195(7) 22_676 ?
Mn1 O25 2.196(9) . ?
Mn1 O12 2.265(7) . ?
Mn2 O24 2.082(7) 11_564 ?
Mn2 O24 2.082(7) . ?
Mn2 O28A 2.11(2) . ?
Mn2 O28A 2.11(2) 11_564 ?
Mn2 O28 2.30(4) . ?
Mn2 O28 2.30(4) 11_564 ?
Mn2 O27 2.168(14) . ?
Mn2 O27 2.168(14) 11_564 ?
Mn3 O30 2.10(2) . ?
Mn3 O29 2.117(19) . ?
Mn3 O5 2.240(8) 22_676 ?
Mn3 O1 2.239(9) . ?
Mn3 O7 2.261(10) 27_556 ?
Mn3 O31 2.29(3) . ?
Mn3 Mn3 3.206(8) 7_556 ?
P1 O3 1.544(6) 7_556 ?
P1 O3 1.544(6) . ?
P1 O4 1.558(7) 7_556 ?
P1 O4 1.558(7) . ?
O1 Mn3 2.239(9) 7_556 ?
O5 Mn3 2.240(8) 30_665 ?
O6 V9 2.027(7) 7_556 ?
O7 Mn3 2.261(10) 27_546 ?
O7 Mn3 2.261(10) 29_545 ?
O8 Mn1 2.195(7) 30_665 ?
O11 V9 1.933(6) 7_556 ?
O13 V3 1.933(7) 7_556 ?
O14 V3 1.927(7) 7_556 ?
O15 V9 1.951(7) 7_556 ?
O20 V7 1.974(7) 7_556 ?
O21 Mn1 2.096(7) 25_566 ?
O23 V7 1.883(6) 7_556 ?
O23 V8 1.927(6) 7_556 ?
O2W O2W 1.28(9) 8_666 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O12 V1 O13 105.7(3) . . ?
O12 V1 O19 103.9(3) . . ?
O13 V1 O19 90.8(3) . . ?
O12 V1 O10 98.0(3) . . ?
O13 V1 O10 82.7(3) . . ?
O19 V1 O10 158.1(3) . . ?
O12 V1 O9 92.4(3) . . ?
O13 V1 O9 161.5(3) . . ?
O19 V1 O9 80.9(3) . . ?
O10 V1 O9 98.9(3) . . ?
O12 V1 O3 161.2(3) . . ?
O13 V1 O3 89.6(3) . . ?
O19 V1 O3 86.5(3) . . ?
O10 V1 O3 72.7(3) . . ?
O9 V1 O3 73.5(2) . . ?
O12 V1 V5 103.3(3) . . ?
O13 V1 V5 126.6(2) . . ?
O19 V1 V5 38.75(19) . . ?
O10 V1 V5 135.5(2) . . ?
O9 V1 V5 42.29(18) . . ?
O3 V1 V5 74.80(16) . . ?
O18 V2 O19 104.1(4) . . ?
O18 V2 O14 105.6(4) . . ?
O19 V2 O14 90.9(3) . . ?
O18 V2 O15 100.7(3) . . ?
O19 V2 O15 82.8(3) . . ?
O14 V2 O15 153.6(3) . . ?
O18 V2 O16 98.1(3) . . ?
O19 V2 O16 157.5(3) . . ?
O14 V2 O16 79.2(3) . . ?
O15 V2 O16 97.0(3) . . ?
O18 V2 V5 105.6(3) . . ?
O19 V2 V5 40.1(2) . . ?
O14 V2 V5 127.0(2) . . ?
O15 V2 V5 42.71(19) . . ?
O16 V2 V5 135.9(2) . . ?
O18 V2 V7 106.3(3) . . ?
O19 V2 V7 124.4(2) . . ?
O14 V2 V7 36.4(2) . . ?
O15 V2 V7 133.6(2) . . ?
O16 V2 V7 42.87(19) . . ?
V5 V2 V7 147.65(8) . . ?
O22 V3 O10 104.1(4) . . ?
O22 V3 O14 104.0(4) . 7_556 ?
O10 V3 O14 151.8(3) . 7_556 ?
O22 V3 O13 103.1(3) . 7_556 ?
O10 V3 O13 81.6(3) . 7_556 ?
O14 V3 O13 89.3(3) 7_556 7_556 ?
O22 V3 O20 100.8(3) . . ?
O10 V3 O20 92.2(3) . . ?
O14 V3 O20 85.4(3) 7_556 . ?
O13 V3 O20 156.1(3) 7_556 . ?
O22 V3 V7 104.6(3) . 7_556 ?
O10 V3 V7 131.4(2) . 7_556 ?
O14 V3 V7 41.3(2) 7_556 7_556 ?
O13 V3 V7 127.7(2) 7_556 7_556 ?
O20 V3 V7 44.2(2) . 7_556 ?
O22 V3 V6 106.9(3) . . ?
O10 V3 V6 41.9(2) . . ?
O14 V3 V6 124.7(2) 7_556 . ?
O13 V3 V6 39.7(2) 7_556 . ?
O20 V3 V6 130.5(2) . . ?
V7 V3 V6 148.30(8) 7_556 . ?
O17 V4 O23 100.9(3) . . ?
O17 V4 O11 101.2(3) . . ?
O23 V4 O11 90.1(3) . . ?
O17 V4 O20 101.3(3) . . ?
O23 V4 O20 84.6(3) . . ?
O11 V4 O20 157.5(3) . . ?
O17 V4 O9 100.4(3) . . ?
O23 V4 O9 158.1(3) . . ?
O11 V4 O9 81.0(3) . . ?
O20 V4 O9 96.0(3) . . ?
O17 V4 O3 171.5(3) . . ?
O23 V4 O3 85.3(2) . . ?
O11 V4 O3 84.4(3) . . ?
O20 V4 O3 73.4(2) . . ?
O9 V4 O3 74.0(2) . . ?
O17 V4 V7 103.8(3) . 7_556 ?
O23 V4 V7 40.96(18) . 7_556 ?
O11 V4 V7 128.1(2) . 7_556 ?
O20 V4 V7 43.7(2) . 7_556 ?
O9 V4 V7 136.1(2) . 7_556 ?
O3 V4 V7 77.11(17) . 7_556 ?
O17 V4 V5 105.5(3) . . ?
O23 V4 V5 125.52(19) . . ?
O11 V4 V5 38.7(2) . . ?
O20 V4 V5 133.4(2) . . ?
O9 V4 V5 42.28(19) . . ?
O3 V4 V5 74.87(17) . . ?
V7 V4 V5 150.09(7) 7_556 . ?
O21 V5 O19 118.3(3) . . ?
O21 V5 O11 117.5(3) . . ?
O19 V5 O11 124.3(3) . . ?
O21 V5 O15 105.3(3) . . ?
O19 V5 O15 82.7(3) . . ?
O11 V5 O15 82.9(3) . . ?
O21 V5 O9 107.9(3) . . ?
O19 V5 O9 82.1(3) . . ?
O11 V5 O9 81.6(3) . . ?
O15 V5 O9 146.8(3) . . ?
O21 V5 V2 118.5(3) . . ?
O19 V5 V2 40.8(2) . . ?
O11 V5 V2 108.2(2) . . ?
O15 V5 V2 41.9(2) . . ?
O9 V5 V2 117.93(19) . . ?
O21 V5 V9 118.1(3) . 7_556 ?
O19 V5 V9 107.9(2) . 7_556 ?
O11 V5 V9 41.02(19) . 7_556 ?
O15 V5 V9 41.90(19) . 7_556 ?
O9 V5 V9 117.5(2) . 7_556 ?
V2 V5 V9 74.16(6) . 7_556 ?
O21 V5 V4 121.7(3) . . ?
O19 V5 V4 105.7(2) . . ?
O11 V5 V4 40.10(19) . . ?
O15 V5 V4 116.8(2) . . ?
O9 V5 V4 41.50(19) . . ?
V2 V5 V4 119.78(7) . . ?
V9 V5 V4 77.84(6) 7_556 . ?
O21 V5 V1 123.8(3) . . ?
O19 V5 V1 39.94(19) . . ?
O11 V5 V1 104.6(2) . . ?
O15 V5 V1 115.7(2) . . ?
O9 V5 V1 42.30(19) . . ?
V2 V5 V1 77.10(6) . . ?
V9 V5 V1 118.11(7) 7_556 . ?
V4 V5 V1 71.09(6) . . ?
O1 V6 O13 116.5(2) . 7_556 ?
O1 V6 O13 116.5(2) . . ?
O13 V6 O13 127.0(4) 7_556 . ?
O1 V6 O10 108.3(2) . . ?
O13 V6 O10 80.7(3) 7_556 . ?
O13 V6 O10 83.1(3) . . ?
O1 V6 O10 108.3(2) . 7_556 ?
O13 V6 O10 83.1(3) 7_556 7_556 ?
O13 V6 O10 80.7(3) . 7_556 ?
O10 V6 O10 143.3(4) . 7_556 ?
O1 V6 V1 120.08(5) . 7_556 ?
O13 V6 V1 41.1(2) 7_556 7_556 ?
O13 V6 V1 107.9(2) . 7_556 ?
O10 V6 V1 115.3(2) . 7_556 ?
O10 V6 V1 42.1(2) 7_556 7_556 ?
O1 V6 V3 118.79(5) . . ?
O13 V6 V3 40.6(2) 7_556 . ?
O13 V6 V3 109.2(2) . . ?
O10 V6 V3 40.1(2) . . ?
O10 V6 V3 117.5(2) 7_556 . ?
V1 V6 V3 78.22(6) 7_556 . ?
O1 V6 V3 118.79(5) . 7_556 ?
O13 V6 V3 109.2(2) 7_556 7_556 ?
O13 V6 V3 40.6(2) . 7_556 ?
O10 V6 V3 117.5(2) . 7_556 ?
O10 V6 V3 40.1(2) 7_556 7_556 ?
V1 V6 V3 73.82(6) 7_556 7_556 ?
V3 V6 V3 122.42(10) . 7_556 ?
O24 V7 O14 119.1(4) . . ?
O24 V7 O23 116.8(4) . 7_556 ?
O14 V7 O23 123.5(3) . 7_556 ?
O24 V7 O20 106.7(4) . 7_556 ?
O14 V7 O20 86.0(3) . 7_556 ?
O23 V7 O20 85.9(3) 7_556 7_556 ?
O24 V7 O16 103.0(4) . . ?
O14 V7 O16 79.9(3) . . ?
O23 V7 O16 80.5(3) 7_556 . ?
O20 V7 O16 150.3(3) 7_556 . ?
O24 V7 V3 119.5(3) . 7_556 ?
O14 V7 V3 42.7(2) . 7_556 ?
O23 V7 V3 111.5(2) 7_556 7_556 ?
O20 V7 V3 43.40(19) 7_556 7_556 ?
O16 V7 V3 119.19(19) . 7_556 ?
O24 V7 V4 119.0(4) . 7_556 ?
O14 V7 V4 110.6(2) . 7_556 ?
O23 V7 V4 42.5(2) 7_556 7_556 ?
O20 V7 V4 43.36(19) 7_556 7_556 ?
O16 V7 V4 119.0(2) . 7_556 ?
V3 V7 V4 76.87(6) 7_556 7_556 ?
O24 V7 V8 118.4(3) . . ?
O14 V7 V8 104.3(2) . . ?
O23 V7 V8 37.90(19) 7_556 . ?
O20 V7 V8 118.5(2) 7_556 . ?
O16 V7 V8 42.69(19) . . ?
V3 V7 V8 122.00(7) 7_556 . ?
V4 V7 V8 77.72(6) 7_556 . ?
O24 V7 V2 118.7(4) . . ?
O14 V7 V2 37.6(2) . . ?
O23 V7 V2 105.6(2) 7_556 . ?
O20 V7 V2 119.0(2) 7_556 . ?
O16 V7 V2 42.39(18) . . ?
V3 V7 V2 78.23(6) 7_556 . ?
V4 V7 V2 122.25(7) 7_556 . ?
V8 V7 V2 73.06(6) . . ?
O8 V8 O2 103.6(3) . . ?
O8 V8 O23 101.4(3) . 7_556 ?
O2 V8 O23 92.5(3) . 7_556 ?
O8 V8 O6 99.7(3) . . ?
O2 V8 O6 83.2(3) . . ?
O23 V8 O6 158.8(3) 7_556 . ?
O8 V8 O16 97.9(3) . . ?
O2 V8 O16 158.3(3) . . ?
O23 V8 O16 80.0(3) 7_556 . ?
O6 V8 O16 96.5(3) . . ?
O8 V8 O4 167.3(3) . . ?
O2 V8 O4 86.3(3) . . ?
O23 V8 O4 85.9(2) 7_556 . ?
O6 V8 O4 73.2(3) . . ?
O16 V8 O4 73.0(2) . . ?
O8 V8 V10 105.4(3) . . ?
O2 V8 V10 39.1(2) . . ?
O23 V8 V10 128.75(19) 7_556 . ?
O6 V8 V10 44.0(2) . . ?
O16 V8 V10 136.5(2) . . ?
O4 V8 V10 77.15(18) . . ?
O8 V8 V7 104.5(3) . . ?
O2 V8 V7 125.9(2) . . ?
O23 V8 V7 36.90(18) 7_556 . ?
O6 V8 V7 134.8(2) . . ?
O16 V8 V7 43.12(19) . . ?
O4 V8 V7 75.10(18) . . ?
V10 V8 V7 149.48(8) . . ?
O5 V9 O11 102.5(3) . 7_556 ?
O5 V9 O2 102.4(3) . . ?
O11 V9 O2 91.9(3) 7_556 . ?
O5 V9 O15 100.6(3) . 7_556 ?
O11 V9 O15 82.6(3) 7_556 7_556 ?
O2 V9 O15 157.0(3) . 7_556 ?
O5 V9 O6 97.3(3) . 7_556 ?
O11 V9 O6 159.9(3) 7_556 7_556 ?
O2 V9 O6 80.7(3) . 7_556 ?
O15 V9 O6 97.0(3) 7_556 7_556 ?
O5 V9 V5 104.5(3) . 7_556 ?
O11 V9 V5 40.0(2) 7_556 7_556 ?
O2 V9 V5 128.6(2) . 7_556 ?
O15 V9 V5 42.64(19) 7_556 7_556 ?
O6 V9 V5 136.5(2) 7_556 7_556 ?
O5 V9 V10 103.2(3) . . ?
O11 V9 V10 127.4(2) 7_556 . ?
O2 V9 V10 37.9(2) . . ?
O15 V9 V10 135.2(2) 7_556 . ?
O6 V9 V10 42.8(2) 7_556 . ?
V5 V9 V10 151.82(8) 7_556 . ?
O7 V10 O2 120.0(2) . 7_556 ?
O7 V10 O2 120.0(2) . . ?
O2 V10 O2 120.0(4) 7_556 . ?
O7 V10 O6 106.2(2) . 7_556 ?
O2 V10 O6 82.6(3) 7_556 7_556 ?
O2 V10 O6 81.4(3) . 7_556 ?
O7 V10 O6 106.2(2) . . ?
O2 V10 O6 81.4(3) 7_556 . ?
O2 V10 O6 82.6(3) . . ?
O6 V10 O6 147.7(4) 7_556 . ?
O7 V10 V8 121.12(6) . 7_556 ?
O2 V10 V8 39.6(2) 7_556 7_556 ?
O2 V10 V8 104.7(2) . 7_556 ?
O6 V10 V8 43.02(19) 7_556 7_556 ?
O6 V10 V8 116.3(2) . 7_556 ?
O7 V10 V8 121.12(6) . . ?
O2 V10 V8 104.7(2) 7_556 . ?
O2 V10 V8 39.6(2) . . ?
O6 V10 V8 116.3(2) 7_556 . ?
O6 V10 V8 43.02(19) . . ?
V8 V10 V8 117.75(11) 7_556 . ?
O7 V10 V9 121.19(5) . 7_556 ?
O2 V10 V9 39.1(2) 7_556 7_556 ?
O2 V10 V9 105.0(2) . 7_556 ?
O6 V10 V9 116.8(2) 7_556 7_556 ?
O6 V10 V9 42.28(19) . 7_556 ?
V8 V10 V9 76.03(6) 7_556 7_556 ?
V8 V10 V9 72.91(6) . 7_556 ?
O7 V10 V9 121.19(5) . . ?
O2 V10 V9 105.0(2) 7_556 . ?
O2 V10 V9 39.1(2) . . ?
O6 V10 V9 42.28(19) 7_556 . ?
O6 V10 V9 116.8(2) . . ?
V8 V10 V9 72.91(6) 7_556 . ?
V8 V10 V9 76.03(6) . . ?
V9 V10 V9 117.62(11) 7_556 . ?
O21 Mn1 O26 93.1(3) 25_566 . ?
O21 Mn1 O9 106.4(3) 25_566 . ?
O26 Mn1 O9 95.4(3) . . ?
O21 Mn1 O8 88.1(3) 25_566 22_676 ?
O26 Mn1 O8 95.6(3) . 22_676 ?
O9 Mn1 O8 161.2(3) . 22_676 ?
O21 Mn1 O25 169.0(3) 25_566 . ?
O26 Mn1 O25 84.9(4) . . ?
O9 Mn1 O25 84.6(3) . . ?
O8 Mn1 O25 81.3(3) 22_676 . ?
O21 Mn1 O12 86.7(3) 25_566 . ?
O26 Mn1 O12 167.9(3) . . ?
O9 Mn1 O12 73.1(2) . . ?
O8 Mn1 O12 96.4(3) 22_676 . ?
O25 Mn1 O12 97.5(3) . . ?
O24 Mn2 O24 178.8(6) 11_564 . ?
O24 Mn2 O28A 89.0(7) 11_564 . ?
O24 Mn2 O28A 91.7(7) . . ?
O24 Mn2 O28A 91.7(7) 11_564 11_564 ?
O24 Mn2 O28A 89.0(7) . 11_564 ?
O28A Mn2 O28A 111.3(15) . 11_564 ?
O24 Mn2 O28 85.2(10) 11_564 . ?
O24 Mn2 O28 95.8(10) . . ?
O28A Mn2 O28 22.6(11) . . ?
O28A Mn2 O28 89.2(14) 11_564 . ?
O24 Mn2 O28 95.8(10) 11_564 11_564 ?
O24 Mn2 O28 85.2(10) . 11_564 ?
O28A Mn2 O28 89.2(14) . 11_564 ?
O28A Mn2 O28 22.6(11) 11_564 11_564 ?
O28 Mn2 O28 68(2) . 11_564 ?
O24 Mn2 O27 95.3(5) 11_564 . ?
O24 Mn2 O27 83.8(5) . . ?
O28A Mn2 O27 79.9(8) . . ?
O28A Mn2 O27 166.9(8) 11_564 . ?
O28 Mn2 O27 102.4(11) . . ?
O28 Mn2 O27 164.2(11) 11_564 . ?
O24 Mn2 O27 83.8(5) 11_564 11_564 ?
O24 Mn2 O27 95.3(5) . 11_564 ?
O28A Mn2 O27 166.9(8) . 11_564 ?
O28A Mn2 O27 79.9(8) 11_564 11_564 ?
O28 Mn2 O27 164.2(11) . 11_564 ?
O28 Mn2 O27 102.4(11) 11_564 11_564 ?
O27 Mn2 O27 89.8(8) . 11_564 ?
O30 Mn3 O29 83.7(10) . . ?
O30 Mn3 O5 90.5(6) . 22_676 ?
O29 Mn3 O5 85.3(5) . 22_676 ?
O30 Mn3 O1 99.7(6) . . ?
O29 Mn3 O1 93.9(6) . . ?
O5 Mn3 O1 169.7(3) 22_676 . ?
O30 Mn3 O7 83.2(8) . 27_556 ?
O29 Mn3 O7 166.8(6) . 27_556 ?
O5 Mn3 O7 93.9(3) 22_676 27_556 ?
O1 Mn3 O7 89.1(4) . 27_556 ?
O30 Mn3 O31 161.8(11) . . ?
O29 Mn3 O31 79.8(9) . . ?
O5 Mn3 O31 80.7(8) 22_676 . ?
O1 Mn3 O31 89.1(8) . . ?
O7 Mn3 O31 113.1(8) 27_556 . ?
O30 Mn3 Mn3 92.0(7) . 7_556 ?
O29 Mn3 Mn3 136.7(5) . 7_556 ?
O5 Mn3 Mn3 137.9(2) 22_676 7_556 ?
O1 Mn3 Mn3 44.3(2) . 7_556 ?
O7 Mn3 Mn3 44.9(3) 27_556 7_556 ?
O31 Mn3 Mn3 105.2(8) . 7_556 ?
O3 P1 O3 110.2(5) 7_556 . ?
O3 P1 O4 110.1(4) 7_556 7_556 ?
O3 P1 O4 109.0(4) . 7_556 ?
O3 P1 O4 109.0(4) 7_556 . ?
O3 P1 O4 110.1(4) . . ?
O4 P1 O4 108.6(6) 7_556 . ?
V6 O1 Mn3 134.3(2) . 7_556 ?
V6 O1 Mn3 134.3(2) . . ?
Mn3 O1 Mn3 91.4(5) 7_556 . ?
V10 O2 V8 101.2(3) . . ?
V10 O2 V9 103.0(3) . . ?
V8 O2 V9 143.4(4) . . ?
P1 O3 V1 129.4(4) . . ?
P1 O3 V4 128.1(4) . . ?
V1 O3 V4 89.9(2) . . ?
P1 O4 V8 128.3(4) . . ?
V9 O5 Mn3 142.9(4) . 30_665 ?
V8 O6 V9 122.1(4) . 7_556 ?
V8 O6 V10 92.9(3) . . ?
V9 O6 V10 94.9(3) 7_556 . ?
V10 O7 Mn3 134.9(3) . 27_546 ?
V10 O7 Mn3 134.9(3) . 29_545 ?
Mn3 O7 Mn3 90.3(5) 27_546 29_545 ?
V8 O8 Mn1 150.6(4) . 30_665 ?
V4 O9 V1 120.0(3) . . ?
V4 O9 V5 96.2(3) . . ?
V1 O9 V5 95.4(3) . . ?
V4 O9 Mn1 129.7(3) . . ?
V1 O9 Mn1 92.2(3) . . ?
V5 O9 Mn1 119.7(3) . . ?
V3 O10 V1 130.2(4) . . ?
V3 O10 V6 98.0(3) . . ?
V1 O10 V6 95.4(3) . . ?
V5 O11 V9 99.0(3) . 7_556 ?
V5 O11 V4 101.2(3) . . ?
V9 O11 V4 144.1(4) 7_556 . ?
V1 O12 Mn1 99.9(3) . . ?
V6 O13 V1 98.8(3) . . ?
V6 O13 V3 99.7(3) . 7_556 ?
V1 O13 V3 144.5(4) . 7_556 ?
V7 O14 V2 106.1(3) . . ?
V7 O14 V3 96.1(3) . 7_556 ?
V2 O14 V3 147.9(4) . 7_556 ?
V2 O15 V9 128.0(4) . 7_556 ?
V2 O15 V5 95.4(3) . . ?
V9 O15 V5 95.5(3) 7_556 . ?
V2 O16 V8 122.7(3) . . ?
V2 O16 V7 94.7(3) . . ?
V8 O16 V7 94.2(3) . . ?
V5 O19 V2 99.0(3) . . ?
V5 O19 V1 101.3(3) . . ?
V2 O19 V1 142.4(4) . . ?
V3 O20 V4 129.4(3) . . ?
V3 O20 V7 92.4(3) . 7_556 ?
V4 O20 V7 93.0(3) . 7_556 ?
V5 O21 Mn1 141.6(4) . 25_566 ?
V7 O23 V8 105.2(3) 7_556 7_556 ?
V7 O23 V4 96.5(3) 7_556 . ?
V8 O23 V4 145.3(3) 7_556 . ?
V7 O24 Mn2 143.1(5) . . ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O18 V2 V5 O21 -7.8(4) . . . . ?
O19 V2 V5 O21 -101.3(4) . . . . ?
O14 V2 V5 O21 -131.9(4) . . . . ?
O15 V2 V5 O21 81.2(4) . . . . ?
O16 V2 V5 O21 112.0(4) . . . . ?
V7 V2 V5 O21 -177.8(3) . . . . ?
O18 V2 V5 O19 93.5(4) . . . . ?
O14 V2 V5 O19 -30.6(4) . . . . ?
O15 V2 V5 O19 -177.5(4) . . . . ?
O16 V2 V5 O19 -146.7(4) . . . . ?
V7 V2 V5 O19 -76.5(3) . . . . ?
O18 V2 V5 O11 -144.8(4) . . . . ?
O19 V2 V5 O11 121.7(4) . . . . ?
O14 V2 V5 O11 91.1(3) . . . . ?
O15 V2 V5 O11 -55.8(3) . . . . ?
O16 V2 V5 O11 -25.0(4) . . . . ?
V7 V2 V5 O11 45.2(3) . . . . ?
O18 V2 V5 O15 -89.0(4) . . . . ?
O19 V2 V5 O15 177.5(4) . . . . ?
O14 V2 V5 O15 146.9(4) . . . . ?
O16 V2 V5 O15 30.8(4) . . . . ?
V7 V2 V5 O15 101.0(3) . . . . ?
O18 V2 V5 O9 125.2(4) . . . . ?
O19 V2 V5 O9 31.7(4) . . . . ?
O14 V2 V5 O9 1.1(3) . . . . ?
O15 V2 V5 O9 -145.8(4) . . . . ?
O16 V2 V5 O9 -115.0(4) . . . . ?
V7 V2 V5 O9 -44.8(3) . . . . ?
O18 V2 V5 V9 -121.6(3) . . . 7_556 ?
O19 V2 V5 V9 144.9(3) . . . 7_556 ?
O14 V2 V5 V9 114.3(3) . . . 7_556 ?
O15 V2 V5 V9 -32.6(3) . . . 7_556 ?
O16 V2 V5 V9 -1.8(3) . . . 7_556 ?
V7 V2 V5 V9 68.37(14) . . . 7_556 ?
O18 V2 V5 V4 172.9(3) . . . . ?
O19 V2 V5 V4 79.4(3) . . . . ?
O14 V2 V5 V4 48.8(3) . . . . ?
O15 V2 V5 V4 -98.1(3) . . . . ?
O16 V2 V5 V4 -67.3(3) . . . . ?
V7 V2 V5 V4 2.87(18) . . . . ?
O18 V2 V5 V1 113.8(3) . . . . ?
O19 V2 V5 V1 20.3(3) . . . . ?
O14 V2 V5 V1 -10.3(3) . . . . ?
O15 V2 V5 V1 -157.2(3) . . . . ?
O16 V2 V5 V1 -126.4(3) . . . . ?
V7 V2 V5 V1 -56.20(14) . . . . ?
O17 V4 V5 O21 -7.5(4) . . . . ?
O23 V4 V5 O21 -123.6(4) . . . . ?
O11 V4 V5 O21 -96.2(4) . . . . ?
O20 V4 V5 O21 115.4(4) . . . . ?
O9 V4 V5 O21 81.1(4) . . . . ?
O3 V4 V5 O21 163.7(3) . . . . ?
V7 V4 V5 O21 -175.2(3) 7_556 . . . ?
O17 V4 V5 O19 -146.3(4) . . . . ?
O23 V4 V5 O19 97.6(3) . . . . ?
O11 V4 V5 O19 125.0(4) . . . . ?
O20 V4 V5 O19 -23.5(4) . . . . ?
O9 V4 V5 O19 -57.8(3) . . . . ?
O3 V4 V5 O19 24.9(3) . . . . ?
V7 V4 V5 O19 45.9(3) 7_556 . . . ?
O17 V4 V5 O11 88.7(4) . . . . ?
O23 V4 V5 O11 -27.4(4) . . . . ?
O20 V4 V5 O11 -148.5(4) . . . . ?
O9 V4 V5 O11 177.2(4) . . . . ?
O3 V4 V5 O11 -100.1(3) . . . . ?
V7 V4 V5 O11 -79.1(3) 7_556 . . . ?
O17 V4 V5 O15 124.0(4) . . . . ?
O23 V4 V5 O15 7.9(3) . . . . ?
O11 V4 V5 O15 35.3(4) . . . . ?
O20 V4 V5 O15 -113.2(3) . . . . ?
O9 V4 V5 O15 -147.5(4) . . . . ?
O3 V4 V5 O15 -64.8(3) . . . . ?
V7 V4 V5 O15 -43.8(3) 7_556 . . . ?
O17 V4 V5 O9 -88.5(4) . . . . ?
O23 V4 V5 O9 155.4(4) . . . . ?
O11 V4 V5 O9 -177.2(4) . . . . ?
O20 V4 V5 O9 34.3(4) . . . . ?
O3 V4 V5 O9 82.7(3) . . . . ?
V7 V4 V5 O9 103.7(3) 7_556 . . . ?
O17 V4 V5 V2 171.8(3) . . . . ?
O23 V4 V5 V2 55.7(2) . . . . ?
O11 V4 V5 V2 83.1(3) . . . . ?
O20 V4 V5 V2 -65.3(3) . . . . ?
O9 V4 V5 V2 -99.7(3) . . . . ?
O3 V4 V5 V2 -17.00(17) . . . . ?
V7 V4 V5 V2 4.04(18) 7_556 . . . ?
O17 V4 V5 V9 108.2(3) . . . 7_556 ?
O23 V4 V5 V9 -7.9(2) . . . 7_556 ?
O11 V4 V5 V9 19.5(3) . . . 7_556 ?
O20 V4 V5 V9 -128.9(3) . . . 7_556 ?
O9 V4 V5 V9 -163.2(3) . . . 7_556 ?
O3 V4 V5 V9 -80.58(16) . . . 7_556 ?
V7 V4 V5 V9 -59.54(15) 7_556 . . 7_556 ?
O17 V4 V5 V1 -126.1(3) . . . . ?
O23 V4 V5 V1 117.8(2) . . . . ?
O11 V4 V5 V1 145.2(3) . . . . ?
O20 V4 V5 V1 -3.2(3) . . . . ?
O9 V4 V5 V1 -37.6(3) . . . . ?
O3 V4 V5 V1 45.10(16) . . . . ?
V7 V4 V5 V1 66.14(14) 7_556 . . . ?
O12 V1 V5 O21 -0.6(4) . . . . ?
O13 V1 V5 O21 120.9(4) . . . . ?
O19 V1 V5 O21 95.1(4) . . . . ?
O10 V1 V5 O21 -117.0(4) . . . . ?
O9 V1 V5 O21 -79.2(4) . . . . ?
O3 V1 V5 O21 -161.2(3) . . . . ?
O12 V1 V5 O19 -95.7(4) . . . . ?
O13 V1 V5 O19 25.8(4) . . . . ?
O10 V1 V5 O19 147.9(4) . . . . ?
O9 V1 V5 O19 -174.3(4) . . . . ?
O3 V1 V5 O19 103.7(4) . . . . ?
O12 V1 V5 O11 137.8(3) . . . . ?
O13 V1 V5 O11 -100.7(3) . . . . ?
O19 V1 V5 O11 -126.5(4) . . . . ?
O10 V1 V5 O11 21.4(4) . . . . ?
O9 V1 V5 O11 59.2(3) . . . . ?
O3 V1 V5 O11 -22.8(3) . . . . ?
O12 V1 V5 O15 -133.1(3) . . . . ?
O13 V1 V5 O15 -11.6(3) . . . . ?
O19 V1 V5 O15 -37.4(4) . . . . ?
O10 V1 V5 O15 110.5(4) . . . . ?
O9 V1 V5 O15 148.3(4) . . . . ?
O3 V1 V5 O15 66.3(3) . . . . ?
O12 V1 V5 O9 78.6(4) . . . . ?
O13 V1 V5 O9 -159.9(4) . . . . ?
O19 V1 V5 O9 174.3(4) . . . . ?
O10 V1 V5 O9 -37.8(4) . . . . ?
O3 V1 V5 O9 -82.0(3) . . . . ?
O12 V1 V5 V2 -116.4(3) . . . . ?
O13 V1 V5 V2 5.1(3) . . . . ?
O19 V1 V5 V2 -20.7(3) . . . . ?
O10 V1 V5 V2 127.2(3) . . . . ?
O9 V1 V5 V2 165.0(3) . . . . ?
O3 V1 V5 V2 82.97(16) . . . . ?
O12 V1 V5 V9 179.7(3) . . . 7_556 ?
O13 V1 V5 V9 -58.8(3) . . . 7_556 ?
O19 V1 V5 V9 -84.6(3) . . . 7_556 ?
O10 V1 V5 V9 63.3(3) . . . 7_556 ?
O9 V1 V5 V9 101.1(3) . . . 7_556 ?
O3 V1 V5 V9 19.06(17) . . . 7_556 ?
O12 V1 V5 V4 115.5(3) . . . . ?
O13 V1 V5 V4 -123.0(3) . . . . ?
O19 V1 V5 V4 -148.8(3) . . . . ?
O10 V1 V5 V4 -0.9(3) . . . . ?
O9 V1 V5 V4 36.9(3) . . . . ?
O3 V1 V5 V4 -45.13(16) . . . . ?
O22 V3 V6 O1 7.8(3) . . . . ?
O10 V3 V6 O1 -84.6(3) . . . . ?
O14 V3 V6 O1 129.0(2) 7_556 . . . ?
O13 V3 V6 O1 98.1(3) 7_556 . . . ?
O20 V3 V6 O1 -113.3(3) . . . . ?
V7 V3 V6 O1 -179.15(12) 7_556 . . . ?
O22 V3 V6 O13 -90.3(4) . . . 7_556 ?
O10 V3 V6 O13 177.3(4) . . . 7_556 ?
O14 V3 V6 O13 30.9(4) 7_556 . . 7_556 ?
O20 V3 V6 O13 148.5(4) . . . 7_556 ?
V7 V3 V6 O13 82.7(3) 7_556 . . 7_556 ?
O22 V3 V6 O13 144.8(4) . . . . ?
O10 V3 V6 O13 52.4(4) . . . . ?
O14 V3 V6 O13 -94.0(3) 7_556 . . . ?
O13 V3 V6 O13 -124.9(5) 7_556 . . . ?
O20 V3 V6 O13 23.6(3) . . . . ?
V7 V3 V6 O13 -42.2(3) 7_556 . . . ?
O22 V3 V6 O10 92.4(4) . . . . ?
O14 V3 V6 O10 -146.4(4) 7_556 . . . ?
O13 V3 V6 O10 -177.3(4) 7_556 . . . ?
O20 V3 V6 O10 -28.8(4) . . . . ?
V7 V3 V6 O10 -94.6(3) 7_556 . . . ?
O22 V3 V6 O10 -125.8(4) . . . 7_556 ?
O10 V3 V6 O10 141.8(4) . . . 7_556 ?
O14 V3 V6 O10 -4.6(3) 7_556 . . 7_556 ?
O13 V3 V6 O10 -35.6(4) 7_556 . . 7_556 ?
O20 V3 V6 O10 113.0(3) . . . 7_556 ?
V7 V3 V6 O10 47.2(3) 7_556 . . 7_556 ?
O22 V3 V6 V1 -110.2(3) . . . 7_556 ?
O10 V3 V6 V1 157.4(3) . . . 7_556 ?
O14 V3 V6 V1 11.0(2) 7_556 . . 7_556 ?
O13 V3 V6 V1 -19.9(3) 7_556 . . 7_556 ?
O20 V3 V6 V1 128.6(3) . . . 7_556 ?
V7 V3 V6 V1 62.84(14) 7_556 . . 7_556 ?
O22 V3 V6 V3 -172.2(3) . . . 7_556 ?
O10 V3 V6 V3 95.4(3) . . . 7_556 ?
O14 V3 V6 V3 -51.0(2) 7_556 . . 7_556 ?
O13 V3 V6 V3 -81.9(3) 7_556 . . 7_556 ?
O20 V3 V6 V3 66.7(3) . . . 7_556 ?
V7 V3 V6 V3 0.85(12) 7_556 . . 7_556 ?
O18 V2 V7 O24 6.9(5) . . . . ?
O19 V2 V7 O24 127.5(4) . . . . ?
O14 V2 V7 O24 101.4(5) . . . . ?
O15 V2 V7 O24 -116.2(4) . . . . ?
O16 V2 V7 O24 -77.3(4) . . . . ?
V5 V2 V7 O24 176.9(3) . . . . ?
O18 V2 V7 O14 -94.4(4) . . . . ?
O19 V2 V7 O14 26.1(4) . . . . ?
O15 V2 V7 O14 142.5(4) . . . . ?
O16 V2 V7 O14 -178.7(4) . . . . ?
V5 V2 V7 O14 75.5(4) . . . . ?
O18 V2 V7 O23 140.3(4) . . . 7_556 ?
O19 V2 V7 O23 -99.2(3) . . . 7_556 ?
O14 V2 V7 O23 -125.3(4) . . . 7_556 ?
O15 V2 V7 O23 17.2(3) . . . 7_556 ?
O16 V2 V7 O23 56.0(3) . . . 7_556 ?
V5 V2 V7 O23 -49.8(3) . . . 7_556 ?
O18 V2 V7 O20 -125.8(4) . . . 7_556 ?
O19 V2 V7 O20 -5.2(3) . . . 7_556 ?
O14 V2 V7 O20 -31.3(4) . . . 7_556 ?
O15 V2 V7 O20 111.1(3) . . . 7_556 ?
O16 V2 V7 O20 149.9(4) . . . 7_556 ?
V5 V2 V7 O20 44.2(3) . . . 7_556 ?
O18 V2 V7 O16 84.3(4) . . . . ?
O19 V2 V7 O16 -155.2(4) . . . . ?
O14 V2 V7 O16 178.7(4) . . . . ?
O15 V2 V7 O16 -38.8(4) . . . . ?
V5 V2 V7 O16 -105.7(3) . . . . ?
O18 V2 V7 V3 -110.4(3) . . . 7_556 ?
O19 V2 V7 V3 10.1(2) . . . 7_556 ?
O14 V2 V7 V3 -16.0(3) . . . 7_556 ?
O15 V2 V7 V3 126.5(3) . . . 7_556 ?
O16 V2 V7 V3 165.3(3) . . . 7_556 ?
V5 V2 V7 V3 59.55(14) . . . 7_556 ?
O18 V2 V7 V4 -176.5(3) . . . 7_556 ?
O19 V2 V7 V4 -56.0(3) . . . 7_556 ?
O14 V2 V7 V4 -82.1(3) . . . 7_556 ?
O15 V2 V7 V4 60.4(3) . . . 7_556 ?
O16 V2 V7 V4 99.2(3) . . . 7_556 ?
V5 V2 V7 V4 -6.52(18) . . . 7_556 ?
O18 V2 V7 V8 120.6(3) . . . . ?
O19 V2 V7 V8 -118.9(2) . . . . ?
O14 V2 V7 V8 -145.0(3) . . . . ?
O15 V2 V7 V8 -2.5(3) . . . . ?
O16 V2 V7 V8 36.3(3) . . . . ?
V5 V2 V7 V8 -69.45(14) . . . . ?
O24 V7 V8 O8 -8.1(5) . . . . ?
O14 V7 V8 O8 -143.2(3) . . . . ?
O23 V7 V8 O8 89.8(4) 7_556 . . . ?
O20 V7 V8 O8 123.6(3) 7_556 . . . ?
O16 V7 V8 O8 -86.0(4) . . . . ?
V3 V7 V8 O8 174.1(3) 7_556 . . . ?
V4 V7 V8 O8 108.3(3) 7_556 . . . ?
V2 V7 V8 O8 -122.1(3) . . . . ?
O24 V7 V8 O2 -127.2(5) . . . . ?
O14 V7 V8 O2 97.7(3) . . . . ?
O23 V7 V8 O2 -29.3(4) 7_556 . . . ?
O20 V7 V8 O2 4.5(4) 7_556 . . . ?
O16 V7 V8 O2 154.9(4) . . . . ?
V3 V7 V8 O2 55.0(3) 7_556 . . . ?
V4 V7 V8 O2 -10.8(3) 7_556 . . . ?
V2 V7 V8 O2 118.8(3) . . . . ?
O24 V7 V8 O23 -97.9(5) . . . 7_556 ?
O14 V7 V8 O23 127.0(4) . . . 7_556 ?
O20 V7 V8 O23 33.8(4) 7_556 . . 7_556 ?
O16 V7 V8 O23 -175.8(4) . . . 7_556 ?
V3 V7 V8 O23 84.3(3) 7_556 . . 7_556 ?
V4 V7 V8 O23 18.5(3) 7_556 . . 7_556 ?
V2 V7 V8 O23 148.1(3) . . . 7_556 ?
O24 V7 V8 O6 112.1(5) . . . . ?
O14 V7 V8 O6 -23.0(4) . . . . ?
O23 V7 V8 O6 -150.0(4) 7_556 . . . ?
O20 V7 V8 O6 -116.2(4) 7_556 . . . ?
O16 V7 V8 O6 34.2(4) . . . . ?
V3 V7 V8 O6 -65.7(3) 7_556 . . . ?
V4 V7 V8 O6 -131.5(3) 7_556 . . . ?
V2 V7 V8 O6 -1.9(3) . . . . ?
O24 V7 V8 O16 77.9(5) . . . . ?
O14 V7 V8 O16 -57.2(3) . . . . ?
O23 V7 V8 O16 175.8(4) 7_556 . . . ?
O20 V7 V8 O16 -150.4(4) 7_556 . . . ?
V3 V7 V8 O16 -99.8(3) 7_556 . . . ?
V4 V7 V8 O16 -165.6(3) 7_556 . . . ?
V2 V7 V8 O16 -36.1(3) . . . . ?
O24 V7 V8 O4 158.7(4) . . . . ?
O14 V7 V8 O4 23.6(3) . . . . ?
O23 V7 V8 O4 -103.3(4) 7_556 . . . ?
O20 V7 V8 O4 -69.5(3) 7_556 . . . ?
O16 V7 V8 O4 80.8(3) . . . . ?
V3 V7 V8 O4 -19.02(19) 7_556 . . . ?
V4 V7 V8 O4 -84.81(18) 7_556 . . . ?
V2 V7 V8 O4 44.77(18) . . . . ?
O24 V7 V8 V10 -176.0(4) . . . . ?
O14 V7 V8 V10 48.9(3) . . . . ?
O23 V7 V8 V10 -78.1(3) 7_556 . . . ?
O20 V7 V8 V10 -44.3(3) 7_556 . . . ?
O16 V7 V8 V10 106.1(3) . . . . ?
V3 V7 V8 V10 6.25(18) 7_556 . . . ?
V4 V7 V8 V10 -59.54(13) 7_556 . . . ?
V2 V7 V8 V10 70.04(13) . . . . ?
O8 V8 V10 O7 8.0(3) . . . . ?
O2 V8 V10 O7 100.7(3) . . . . ?
O23 V8 V10 O7 126.9(2) 7_556 . . . ?
O6 V8 V10 O7 -80.2(3) . . . . ?
O16 V8 V10 O7 -111.7(3) . . . . ?
O4 V8 V10 O7 -159.17(17) . . . . ?
V7 V8 V10 O7 175.80(11) . . . . ?
O8 V8 V10 O2 147.6(4) . . . 7_556 ?
O2 V8 V10 O2 -119.7(5) . . . 7_556 ?
O23 V8 V10 O2 -93.4(3) 7_556 . . 7_556 ?
O6 V8 V10 O2 59.4(4) . . . 7_556 ?
O16 V8 V10 O2 27.9(4) . . . 7_556 ?
O4 V8 V10 O2 -19.6(3) . . . 7_556 ?
V7 V8 V10 O2 -44.6(2) . . . 7_556 ?
O8 V8 V10 O2 -92.8(4) . . . . ?
O23 V8 V10 O2 26.2(4) 7_556 . . . ?
O6 V8 V10 O2 179.1(4) . . . . ?
O16 V8 V10 O2 147.5(4) . . . . ?
O4 V8 V10 O2 100.1(4) . . . . ?
V7 V8 V10 O2 75.1(3) . . . . ?
O8 V8 V10 O6 -123.5(3) . . . 7_556 ?
O2 V8 V10 O6 -30.7(4) . . . 7_556 ?
O23 V8 V10 O6 -4.5(3) 7_556 . . 7_556 ?
O6 V8 V10 O6 148.4(4) . . . 7_556 ?
O16 V8 V10 O6 116.9(4) . . . 7_556 ?
O4 V8 V10 O6 69.4(3) . . . 7_556 ?
V7 V8 V10 O6 44.4(3) . . . 7_556 ?
O8 V8 V10 O6 88.1(4) . . . . ?
O2 V8 V10 O6 -179.1(4) . . . . ?
O23 V8 V10 O6 -152.9(4) 7_556 . . . ?
O16 V8 V10 O6 -31.6(4) . . . . ?
O4 V8 V10 O6 -79.0(3) . . . . ?
V7 V8 V10 O6 -104.0(3) . . . . ?
O8 V8 V10 V8 -172.0(3) . . . 7_556 ?
O2 V8 V10 V8 -79.3(3) . . . 7_556 ?
O23 V8 V10 V8 -53.1(2) 7_556 . . 7_556 ?
O6 V8 V10 V8 99.8(3) . . . 7_556 ?
O16 V8 V10 V8 68.3(3) . . . 7_556 ?
O4 V8 V10 V8 20.83(17) . . . 7_556 ?
V7 V8 V10 V8 -4.20(11) . . . 7_556 ?
O8 V8 V10 V9 124.5(3) . . . 7_556 ?
O2 V8 V10 V9 -142.7(3) . . . 7_556 ?
O23 V8 V10 V9 -116.5(2) 7_556 . . 7_556 ?
O6 V8 V10 V9 36.4(3) . . . 7_556 ?
O16 V8 V10 V9 4.8(3) . . . 7_556 ?
O4 V8 V10 V9 -42.61(18) . . . 7_556 ?
V7 V8 V10 V9 -67.64(13) . . . 7_556 ?
O8 V8 V10 V9 -110.3(3) . . . . ?
O2 V8 V10 V9 -17.5(3) . . . . ?
O23 V8 V10 V9 8.7(3) 7_556 . . . ?
O6 V8 V10 V9 161.6(3) . . . . ?
O16 V8 V10 V9 130.0(3) . . . . ?
O4 V8 V10 V9 82.59(18) . . . . ?
V7 V8 V10 V9 57.56(13) . . . . ?
O5 V9 V10 O7 -7.1(3) . . . . ?
O11 V9 V10 O7 -124.3(3) 7_556 . . . ?
O2 V9 V10 O7 -100.4(3) . . . . ?
O15 V9 V10 O7 113.1(3) 7_556 . . . ?
O6 V9 V10 O7 79.5(3) 7_556 . . . ?
V5 V9 V10 O7 -176.19(12) 7_556 . . . ?
O5 V9 V10 O2 -147.1(3) . . . 7_556 ?
O11 V9 V10 O2 95.6(3) 7_556 . . 7_556 ?
O2 V9 V10 O2 119.5(5) . . . 7_556 ?
O15 V9 V10 O2 -27.0(4) 7_556 . . 7_556 ?
O6 V9 V10 O2 -60.6(4) 7_556 . . 7_556 ?
V5 V9 V10 O2 43.7(3) 7_556 . . 7_556 ?
O5 V9 V10 O2 93.4(4) . . . . ?
O11 V9 V10 O2 -23.9(4) 7_556 . . . ?
O15 V9 V10 O2 -146.4(4) 7_556 . . . ?
O6 V9 V10 O2 179.9(4) 7_556 . . . ?
V5 V9 V10 O2 -75.7(3) 7_556 . . . ?
O5 V9 V10 O6 -86.6(4) . . . 7_556 ?
O11 V9 V10 O6 156.2(4) 7_556 . . 7_556 ?
O2 V9 V10 O6 -179.9(4) . . . 7_556 ?
O15 V9 V10 O6 33.6(4) 7_556 . . 7_556 ?
V5 V9 V10 O6 104.3(3) 7_556 . . 7_556 ?
O5 V9 V10 O6 125.1(3) . . . . ?
O11 V9 V10 O6 7.9(4) 7_556 . . . ?
O2 V9 V10 O6 31.7(4) . . . . ?
O15 V9 V10 O6 -114.7(4) 7_556 . . . ?
O6 V9 V10 O6 -148.3(4) 7_556 . . . ?
V5 V9 V10 O6 -44.0(3) 7_556 . . . ?
O5 V9 V10 V8 -123.6(3) . . . 7_556 ?
O11 V9 V10 V8 119.2(3) 7_556 . . 7_556 ?
O2 V9 V10 V8 143.1(3) . . . 7_556 ?
O15 V9 V10 V8 -3.4(3) 7_556 . . 7_556 ?
O6 V9 V10 V8 -37.0(3) 7_556 . . 7_556 ?
V5 V9 V10 V8 67.32(14) 7_556 . . 7_556 ?
O5 V9 V10 V8 111.1(3) . . . . ?
O11 V9 V10 V8 -6.1(3) 7_556 . . . ?
O2 V9 V10 V8 17.7(3) . . . . ?
O15 V9 V10 V8 -128.7(3) 7_556 . . . ?
O6 V9 V10 V8 -162.3(3) 7_556 . . . ?
V5 V9 V10 V8 -58.03(14) 7_556 . . . ?
O5 V9 V10 V9 172.9(3) . . . 7_556 ?
O11 V9 V10 V9 55.7(3) 7_556 . . 7_556 ?
O2 V9 V10 V9 79.6(3) . . . 7_556 ?
O15 V9 V10 V9 -66.9(3) 7_556 . . 7_556 ?
O6 V9 V10 V9 -100.5(3) 7_556 . . 7_556 ?
V5 V9 V10 V9 3.81(12) 7_556 . . 7_556 ?
O13 V6 O1 Mn3 -96.5(3) 7_556 . . 7_556 ?
O13 V6 O1 Mn3 83.5(3) . . . 7_556 ?
O10 V6 O1 Mn3 174.9(3) . . . 7_556 ?
O10 V6 O1 Mn3 -5.1(3) 7_556 . . 7_556 ?
V1 V6 O1 Mn3 -49.69(17) 7_556 . . 7_556 ?
V3 V6 O1 Mn3 -142.51(17) . . . 7_556 ?
V3 V6 O1 Mn3 37.49(17) 7_556 . . 7_556 ?
O13 V6 O1 Mn3 83.5(3) 7_556 . . . ?
O13 V6 O1 Mn3 -96.5(3) . . . . ?
O10 V6 O1 Mn3 -5.1(3) . . . . ?
O10 V6 O1 Mn3 174.9(3) 7_556 . . . ?
V1 V6 O1 Mn3 130.31(17) 7_556 . . . ?
V3 V6 O1 Mn3 37.49(17) . . . . ?
V3 V6 O1 Mn3 -142.51(17) 7_556 . . . ?
O30 Mn3 O1 V6 -97.1(8) . . . . ?
O29 Mn3 O1 V6 -12.8(6) . . . . ?
O5 Mn3 O1 V6 72.7(19) 22_676 . . . ?
O7 Mn3 O1 V6 180.000(1) 27_556 . . . ?
O31 Mn3 O1 V6 66.9(8) . . . . ?
Mn3 Mn3 O1 V6 180.000(2) 7_556 . . . ?
O30 Mn3 O1 Mn3 82.9(8) . . . 7_556 ?
O29 Mn3 O1 Mn3 167.2(6) . . . 7_556 ?
O5 Mn3 O1 Mn3 -107.3(19) 22_676 . . 7_556 ?
O7 Mn3 O1 Mn3 0.0 27_556 . . 7_556 ?
O31 Mn3 O1 Mn3 -113.1(8) . . . 7_556 ?
O7 V10 O2 V8 -103.8(2) . . . . ?
O2 V10 O2 V8 76.2(2) 7_556 . . . ?
O6 V10 O2 V8 152.4(3) 7_556 . . . ?
O6 V10 O2 V8 0.6(3) . . . . ?
V8 V10 O2 V8 116.0(2) 7_556 . . . ?
V9 V10 O2 V8 36.8(3) 7_556 . . . ?
V9 V10 O2 V8 152.4(5) . . . . ?
O7 V10 O2 V9 103.8(2) . . . . ?
O2 V10 O2 V9 -76.2(2) 7_556 . . . ?
O6 V10 O2 V9 0.0(3) 7_556 . . . ?
O6 V10 O2 V9 -151.8(3) . . . . ?
V8 V10 O2 V9 -36.4(3) 7_556 . . . ?
V8 V10 O2 V9 -152.4(5) . . . . ?
V9 V10 O2 V9 -115.6(2) 7_556 . . . ?
O8 V8 O2 V10 97.8(4) . . . . ?
O23 V8 O2 V10 -159.8(3) 7_556 . . . ?
O6 V8 O2 V10 -0.6(3) . . . . ?
O16 V8 O2 V10 -91.0(8) . . . . ?
O4 V8 O2 V10 -74.1(3) . . . . ?
V7 V8 O2 V10 -142.74(19) . . . . ?
O8 V8 O2 V9 -131.4(6) . . . . ?
O23 V8 O2 V9 -29.0(6) 7_556 . . . ?
O6 V8 O2 V9 130.2(6) . . . . ?
O16 V8 O2 V9 39.8(12) . . . . ?
O4 V8 O2 V9 56.7(6) . . . . ?
V10 V8 O2 V9 130.8(8) . . . . ?
V7 V8 O2 V9 -11.9(7) . . . . ?
O5 V9 O2 V10 -95.6(4) . . . . ?
O11 V9 O2 V10 161.2(3) 7_556 . . . ?
O15 V9 O2 V10 86.0(7) 7_556 . . . ?
O6 V9 O2 V10 0.0(3) 7_556 . . . ?
V5 V9 O2 V10 144.13(19) 7_556 . . . ?
O5 V9 O2 V8 134.1(6) . . . . ?
O11 V9 O2 V8 30.9(6) 7_556 . . . ?
O15 V9 O2 V8 -44.4(11) 7_556 . . . ?
O6 V9 O2 V8 -130.4(7) 7_556 . . . ?
V5 V9 O2 V8 13.8(8) 7_556 . . . ?
V10 V9 O2 V8 -130.4(8) . . . . ?
O3 P1 O3 V1 -57.2(3) 7_556 . . . ?
O4 P1 O3 V1 -178.1(4) 7_556 . . . ?
O4 P1 O3 V1 63.0(6) . . . . ?
O3 P1 O3 V4 173.0(6) 7_556 . . . ?
O4 P1 O3 V4 52.2(5) 7_556 . . . ?
O4 P1 O3 V4 -66.8(5) . . . . ?
O12 V1 O3 P1 -175.1(8) . . . . ?
O13 V1 O3 P1 40.1(5) . . . . ?
O19 V1 O3 P1 -50.7(5) . . . . ?
O10 V1 O3 P1 122.5(5) . . . . ?
O9 V1 O3 P1 -132.3(5) . . . . ?
V5 V1 O3 P1 -88.3(5) . . . . ?
O12 V1 O3 V4 -32.3(10) . . . . ?
O13 V1 O3 V4 -177.2(3) . . . . ?
O19 V1 O3 V4 92.0(2) . . . . ?
O10 V1 O3 V4 -94.7(3) . . . . ?
O9 V1 O3 V4 10.5(2) . . . . ?
V5 V1 O3 V4 54.48(15) . . . . ?
O17 V4 O3 P1 -177(2) . . . . ?
O23 V4 O3 P1 -39.8(5) . . . . ?
O11 V4 O3 P1 50.7(5) . . . . ?
O20 V4 O3 P1 -125.5(5) . . . . ?
O9 V4 O3 P1 132.9(5) . . . . ?
V7 V4 O3 P1 -80.4(4) 7_556 . . . ?
V5 V4 O3 P1 89.0(5) . . . . ?
O17 V4 O3 V1 39(2) . . . . ?
O23 V4 O3 V1 176.7(2) . . . . ?
O11 V4 O3 V1 -92.8(3) . . . . ?
O20 V4 O3 V1 90.9(3) . . . . ?
O9 V4 O3 V1 -10.6(2) . . . . ?
V7 V4 O3 V1 136.02(19) 7_556 . . . ?
V5 V4 O3 V1 -54.56(15) . . . . ?
O3 P1 O4 V8 -58.3(6) 7_556 . . . ?
O3 P1 O4 V8 -179.2(4) . . . . ?
O4 P1 O4 V8 61.6(4) 7_556 . . . ?
O8 V8 O4 P1 174.1(12) . . . . ?
O2 V8 O4 P1 -44.4(5) . . . . ?
O23 V8 O4 P1 48.4(5) 7_556 . . . ?
O6 V8 O4 P1 -128.4(6) . . . . ?
O16 V8 O4 P1 129.1(5) . . . . ?
V10 V8 O4 P1 -82.9(5) . . . . ?
V7 V8 O4 P1 84.2(5) . . . . ?
O11 V9 O5 Mn3 36.8(8) 7_556 . . 30_665 ?
O2 V9 O5 Mn3 -57.9(8) . . . 30_665 ?
O15 V9 O5 Mn3 121.5(7) 7_556 . . 30_665 ?
O6 V9 O5 Mn3 -139.9(7) 7_556 . . 30_665 ?
V5 V9 O5 Mn3 77.9(7) 7_556 . . 30_665 ?
V10 V9 O5 Mn3 -96.8(7) . . . 30_665 ?
O8 V8 O6 V9 160.2(4) . . . 7_556 ?
O2 V8 O6 V9 -97.1(4) . . . 7_556 ?
O23 V8 O6 V9 -17.9(10) 7_556 . . 7_556 ?
O16 V8 O6 V9 61.1(4) . . . 7_556 ?
O4 V8 O6 V9 -8.9(3) . . . 7_556 ?
V10 V8 O6 V9 -97.7(4) . . . 7_556 ?
V7 V8 O6 V9 38.3(5) . . . 7_556 ?
O8 V8 O6 V10 -102.1(3) . . . . ?
O2 V8 O6 V10 0.6(3) . . . . ?
O23 V8 O6 V10 79.8(8) 7_556 . . . ?
O16 V8 O6 V10 158.7(3) . . . . ?
O4 V8 O6 V10 88.8(3) . . . . ?
V7 V8 O6 V10 136.0(2) . . . . ?
O7 V10 O6 V8 118.57(19) . . . . ?
O2 V10 O6 V8 -122.6(3) 7_556 . . . ?
O2 V10 O6 V8 -0.6(3) . . . . ?
O6 V10 O6 V8 -61.43(19) 7_556 . . . ?
V8 V10 O6 V8 -103.4(2) 7_556 . . . ?
V9 V10 O6 V8 -122.6(4) 7_556 . . . ?
V9 V10 O6 V8 -20.1(3) . . . . ?
O7 V10 O6 V9 -118.86(19) . . . 7_556 ?
O2 V10 O6 V9 0.0(3) 7_556 . . 7_556 ?
O2 V10 O6 V9 122.0(3) . . . 7_556 ?
O6 V10 O6 V9 61.1(2) 7_556 . . 7_556 ?
V8 V10 O6 V9 19.2(3) 7_556 . . 7_556 ?
V8 V10 O6 V9 122.6(4) . . . 7_556 ?
V9 V10 O6 V9 102.5(2) . . . 7_556 ?
O2 V10 O7 Mn3 88.6(3) 7_556 . . 27_546 ?
O2 V10 O7 Mn3 -91.4(3) . . . 27_546 ?
O6 V10 O7 Mn3 -2.2(3) 7_556 . . 27_546 ?
O6 V10 O7 Mn3 177.8(3) . . . 27_546 ?
V8 V10 O7 Mn3 42.26(17) 7_556 . . 27_546 ?
V8 V10 O7 Mn3 -137.74(17) . . . 27_546 ?
V9 V10 O7 Mn3 134.32(17) 7_556 . . 27_546 ?
V9 V10 O7 Mn3 -45.68(17) . . . 27_546 ?
O2 V10 O7 Mn3 -91.4(3) 7_556 . . 29_545 ?
O2 V10 O7 Mn3 88.6(3) . . . 29_545 ?
O6 V10 O7 Mn3 177.8(3) 7_556 . . 29_545 ?
O6 V10 O7 Mn3 -2.2(3) . . . 29_545 ?
V8 V10 O7 Mn3 -137.74(17) 7_556 . . 29_545 ?
V8 V10 O7 Mn3 42.26(17) . . . 29_545 ?
V9 V10 O7 Mn3 -45.68(17) 7_556 . . 29_545 ?
V9 V10 O7 Mn3 134.32(17) . . . 29_545 ?
O2 V8 O8 Mn1 110.6(9) . . . 30_665 ?
O23 V8 O8 Mn1 15.1(9) 7_556 . . 30_665 ?
O6 V8 O8 Mn1 -164.2(8) . . . 30_665 ?
O16 V8 O8 Mn1 -66.2(9) . . . 30_665 ?
O4 V8 O8 Mn1 -109.2(14) . . . 30_665 ?
V10 V8 O8 Mn1 151.0(8) . . . 30_665 ?
V7 V8 O8 Mn1 -22.7(9) . . . 30_665 ?
O17 V4 O9 V1 -158.5(4) . . . . ?
O23 V4 O9 V1 34.7(9) . . . . ?
O11 V4 O9 V1 101.7(4) . . . . ?
O20 V4 O9 V1 -55.8(4) . . . . ?
O3 V4 O9 V1 15.0(3) . . . . ?
V7 V4 O9 V1 -35.7(5) 7_556 . . . ?
V5 V4 O9 V1 99.9(4) . . . . ?
O17 V4 O9 V5 101.6(3) . . . . ?
O23 V4 O9 V5 -65.2(8) . . . . ?
O11 V4 O9 V5 1.8(3) . . . . ?
O20 V4 O9 V5 -155.7(3) . . . . ?
O3 V4 O9 V5 -85.0(3) . . . . ?
V7 V4 O9 V5 -135.66(19) 7_556 . . . ?
O17 V4 O9 Mn1 -35.9(5) . . . . ?
O23 V4 O9 Mn1 157.3(5) . . . . ?
O11 V4 O9 Mn1 -135.8(4) . . . . ?
O20 V4 O9 Mn1 66.8(4) . . . . ?
O3 V4 O9 Mn1 137.5(5) . . . . ?
V7 V4 O9 Mn1 86.8(4) 7_556 . . . ?
V5 V4 O9 Mn1 -137.5(5) . . . . ?
O12 V1 O9 V4 152.3(4) . . . . ?
O13 V1 O9 V4 -39.8(10) . . . . ?
O19 V1 O9 V4 -104.0(4) . . . . ?
O10 V1 O9 V4 53.9(4) . . . . ?
O3 V1 O9 V4 -15.0(3) . . . . ?
V5 V1 O9 V4 -100.4(4) . . . . ?
O12 V1 O9 V5 -107.3(3) . . . . ?
O13 V1 O9 V5 60.6(9) . . . . ?
O19 V1 O9 V5 -3.6(3) . . . . ?
O10 V1 O9 V5 154.2(3) . . . . ?
O3 V1 O9 V5 85.4(3) . . . . ?
O12 V1 O9 Mn1 12.8(3) . . . . ?
O13 V1 O9 Mn1 -179.3(8) . . . . ?
O19 V1 O9 Mn1 116.5(3) . . . . ?
O10 V1 O9 Mn1 -85.7(3) . . . . ?
O3 V1 O9 Mn1 -154.5(3) . . . . ?
V5 V1 O9 Mn1 120.1(3) . . . . ?
O21 V5 O9 V4 -118.0(3) . . . . ?
O19 V5 O9 V4 124.7(3) . . . . ?
O11 V5 O9 V4 -1.8(3) . . . . ?
O15 V5 O9 V4 61.1(6) . . . . ?
V2 V5 O9 V4 104.4(2) . . . . ?
V9 V5 O9 V4 18.5(3) 7_556 . . . ?
V1 V5 O9 V4 121.0(3) . . . . ?
O21 V5 O9 V1 120.9(3) . . . . ?
O19 V5 O9 V1 3.7(3) . . . . ?
O11 V5 O9 V1 -122.8(3) . . . . ?
O15 V5 O9 V1 -59.9(6) . . . . ?
V2 V5 O9 V1 -16.6(3) . . . . ?
V9 V5 O9 V1 -102.5(2) 7_556 . . . ?
V4 V5 O9 V1 -121.0(3) . . . . ?
O21 V5 O9 Mn1 25.3(4) . . . . ?
O19 V5 O9 Mn1 -92.0(4) . . . . ?
O11 V5 O9 Mn1 141.5(4) . . . . ?
O15 V5 O9 Mn1 -155.6(4) . . . . ?
V2 V5 O9 Mn1 -112.3(3) . . . . ?
V9 V5 O9 Mn1 161.9(2) 7_556 . . . ?
V4 V5 O9 Mn1 143.3(5) . . . . ?
V1 V5 O9 Mn1 -95.7(4) . . . . ?
O21 Mn1 O9 V4 136.0(4) 25_566 . . . ?
O26 Mn1 O9 V4 41.2(5) . . . . ?
O8 Mn1 O9 V4 -84.7(9) 22_676 . . . ?
O25 Mn1 O9 V4 -43.2(5) . . . . ?
O12 Mn1 O9 V4 -142.8(5) . . . . ?
O21 Mn1 O9 V1 -90.9(3) 25_566 . . . ?
O26 Mn1 O9 V1 174.2(3) . . . . ?
O8 Mn1 O9 V1 48.4(9) 22_676 . . . ?
O25 Mn1 O9 V1 89.9(3) . . . . ?
O12 Mn1 O9 V1 -9.7(2) . . . . ?
O21 Mn1 O9 V5 6.6(4) 25_566 . . . ?
O26 Mn1 O9 V5 -88.3(4) . . . . ?
O8 Mn1 O9 V5 145.9(7) 22_676 . . . ?
O25 Mn1 O9 V5 -172.6(4) . . . . ?
O12 Mn1 O9 V5 87.8(4) . . . . ?
O22 V3 O10 V1 156.2(5) . . . . ?
O14 V3 O10 V1 -29.8(9) 7_556 . . . ?
O13 V3 O10 V1 -102.3(5) 7_556 . . . ?
O20 V3 O10 V1 54.5(5) . . . . ?
V7 V3 O10 V1 31.7(6) 7_556 . . . ?
V6 V3 O10 V1 -104.0(5) . . . . ?
O22 V3 O10 V6 -99.8(4) . . . . ?
O14 V3 O10 V6 74.2(6) 7_556 . . . ?
O13 V3 O10 V6 1.7(3) 7_556 . . . ?
O20 V3 O10 V6 158.5(3) . . . . ?
V7 V3 O10 V6 135.72(19) 7_556 . . . ?
O12 V1 O10 V3 -150.7(5) . . . . ?
O13 V1 O10 V3 104.4(5) . . . . ?
O19 V1 O10 V3 30.8(10) . . . . ?
O9 V1 O10 V3 -57.0(5) . . . . ?
O3 V1 O10 V3 12.5(4) . . . . ?
V5 V1 O10 V3 -32.3(6) . . . . ?
O12 V1 O10 V6 104.1(3) . . . . ?
O13 V1 O10 V6 -0.8(3) . . . . ?
O19 V1 O10 V6 -74.4(8) . . . . ?
O9 V1 O10 V6 -162.2(3) . . . . ?
O3 V1 O10 V6 -92.7(3) . . . . ?
V5 V1 O10 V6 -137.52(19) . . . . ?
O1 V6 O10 V3 113.2(2) . . . . ?
O13 V6 O10 V3 -1.8(3) 7_556 . . . ?
O13 V6 O10 V3 -131.1(3) . . . . ?
O10 V6 O10 V3 -66.8(2) 7_556 . . . ?
V1 V6 O10 V3 -24.6(3) 7_556 . . . ?
V3 V6 O10 V3 -108.7(2) 7_556 . . . ?
O1 V6 O10 V1 -114.9(2) . . . . ?
O13 V6 O10 V1 130.2(3) 7_556 . . . ?
O13 V6 O10 V1 0.8(3) . . . . ?
O10 V6 O10 V1 65.1(2) 7_556 . . . ?
V1 V6 O10 V1 107.4(2) 7_556 . . . ?
V3 V6 O10 V1 131.9(4) . . . . ?
V3 V6 O10 V1 23.2(3) 7_556 . . . ?
O21 V5 O11 V9 -102.2(4) . . . 7_556 ?
O19 V5 O11 V9 77.6(4) . . . 7_556 ?
O15 V5 O11 V9 1.4(3) . . . 7_556 ?
O9 V5 O11 V9 152.0(3) . . . 7_556 ?
V2 V5 O11 V9 35.2(3) . . . 7_556 ?
V4 V5 O11 V9 150.1(5) . . . 7_556 ?
V1 V5 O11 V9 116.2(2) . . . 7_556 ?
O21 V5 O11 V4 107.7(4) . . . . ?
O19 V5 O11 V4 -72.5(4) . . . . ?
O15 V5 O11 V4 -148.7(3) . . . . ?
O9 V5 O11 V4 1.9(3) . . . . ?
V2 V5 O11 V4 -114.9(2) . . . . ?
V9 V5 O11 V4 -150.1(5) 7_556 . . . ?
V1 V5 O11 V4 -33.9(3) . . . . ?
O17 V4 O11 V5 -100.8(4) . . . . ?
O23 V4 O11 V5 158.0(3) . . . . ?
O20 V4 O11 V5 82.1(8) . . . . ?
O9 V4 O11 V5 -1.9(3) . . . . ?
O3 V4 O11 V5 72.7(3) . . . . ?
V7 V4 O11 V5 141.52(18) 7_556 . . . ?
O17 V4 O11 V9 136.2(6) . . . 7_556 ?
O23 V4 O11 V9 35.0(6) . . . 7_556 ?
O20 V4 O11 V9 -40.9(11) . . . 7_556 ?
O9 V4 O11 V9 -124.9(6) . . . 7_556 ?
O3 V4 O11 V9 -50.3(6) . . . 7_556 ?
V7 V4 O11 V9 18.5(8) 7_556 . . 7_556 ?
V5 V4 O11 V9 -123.0(8) . . . 7_556 ?
O13 V1 O12 Mn1 171.5(3) . . . . ?
O19 V1 O12 Mn1 -93.7(3) . . . . ?
O10 V1 O12 Mn1 86.8(3) . . . . ?
O9 V1 O12 Mn1 -12.5(3) . . . . ?
O3 V1 O12 Mn1 28.2(11) . . . . ?
V5 V1 O12 Mn1 -53.8(3) . . . . ?
O21 Mn1 O12 V1 120.2(4) 25_566 . . . ?
O26 Mn1 O12 V1 31.0(16) . . . . ?
O9 Mn1 O12 V1 12.0(3) . . . . ?
O8 Mn1 O12 V1 -152.1(3) 22_676 . . . ?
O25 Mn1 O12 V1 -70.0(4) . . . . ?
O1 V6 O13 V1 106.3(2) . . . . ?
O13 V6 O13 V1 -73.7(2) 7_556 . . . ?
O10 V6 O13 V1 -0.8(3) . . . . ?
O10 V6 O13 V1 -147.8(3) 7_556 . . . ?
V1 V6 O13 V1 -115.2(2) 7_556 . . . ?
V3 V6 O13 V1 -31.8(3) . . . . ?
V3 V6 O13 V1 -149.5(5) 7_556 . . . ?
O1 V6 O13 V3 -104.2(2) . . . 7_556 ?
O13 V6 O13 V3 75.8(2) 7_556 . . 7_556 ?
O10 V6 O13 V3 148.7(3) . . . 7_556 ?
O10 V6 O13 V3 1.8(3) 7_556 . . 7_556 ?
V1 V6 O13 V3 34.3(3) 7_556 . . 7_556 ?
V3 V6 O13 V3 117.7(2) . . . 7_556 ?
O12 V1 O13 V6 -95.5(4) . . . . ?
O19 V1 O13 V6 159.9(3) . . . . ?
O10 V1 O13 V6 0.8(3) . . . . ?
O9 V1 O13 V6 97.1(9) . . . . ?
O3 V1 O13 V6 73.4(3) . . . . ?
V5 V1 O13 V6 144.05(18) . . . . ?
O12 V1 O13 V3 144.0(6) . . . 7_556 ?
O19 V1 O13 V3 39.3(7) . . . 7_556 ?
O10 V1 O13 V3 -119.7(7) . . . 7_556 ?
O9 V1 O13 V3 -23.4(14) . . . 7_556 ?
O3 V1 O13 V3 -47.1(7) . . . 7_556 ?
V5 V1 O13 V3 23.5(8) . . . 7_556 ?
O24 V7 O14 V2 -100.3(5) . . . . ?
O23 V7 O14 V2 70.6(4) 7_556 . . . ?
O20 V7 O14 V2 152.9(3) 7_556 . . . ?
O16 V7 O14 V2 -0.9(3) . . . . ?
V3 V7 O14 V2 156.5(5) 7_556 . . . ?
V4 V7 O14 V2 116.5(2) 7_556 . . . ?
V8 V7 O14 V2 34.5(3) . . . . ?
O24 V7 O14 V3 103.2(4) . . . 7_556 ?
O23 V7 O14 V3 -86.0(4) 7_556 . . 7_556 ?
O20 V7 O14 V3 -3.7(3) 7_556 . . 7_556 ?
O16 V7 O14 V3 -157.4(3) . . . 7_556 ?
V4 V7 O14 V3 -40.0(3) 7_556 . . 7_556 ?
V8 V7 O14 V3 -122.1(2) . . . 7_556 ?
V2 V7 O14 V3 -156.5(5) . . . 7_556 ?
O18 V2 O14 V7 96.3(4) . . . . ?
O19 V2 O14 V7 -158.7(3) . . . . ?
O15 V2 O14 V7 -83.1(7) . . . . ?
O16 V2 O14 V7 0.9(3) . . . . ?
V5 V2 O14 V7 -139.6(2) . . . . ?
O18 V2 O14 V3 -131.8(7) . . . 7_556 ?
O19 V2 O14 V3 -26.9(7) . . . 7_556 ?
O15 V2 O14 V3 48.7(11) . . . 7_556 ?
O16 V2 O14 V3 132.7(7) . . . 7_556 ?
V5 V2 O14 V3 -7.8(8) . . . 7_556 ?
V7 V2 O14 V3 131.8(9) . . . 7_556 ?
O18 V2 O15 V9 -157.3(5) . . . 7_556 ?
O19 V2 O15 V9 99.6(4) . . . 7_556 ?
O14 V2 O15 V9 22.2(9) . . . 7_556 ?
O16 V2 O15 V9 -57.7(4) . . . 7_556 ?
V5 V2 O15 V9 101.2(5) . . . 7_556 ?
V7 V2 O15 V9 -32.3(6) . . . 7_556 ?
O18 V2 O15 V5 101.5(4) . . . . ?
O19 V2 O15 V5 -1.6(3) . . . . ?
O14 V2 O15 V5 -79.1(7) . . . . ?
O16 V2 O15 V5 -158.9(3) . . . . ?
V7 V2 O15 V5 -133.48(19) . . . . ?
O21 V5 O15 V2 -115.8(3) . . . . ?
O19 V5 O15 V2 1.6(3) . . . . ?
O11 V5 O15 V2 127.7(3) . . . . ?
O9 V5 O15 V2 65.1(6) . . . . ?
V9 V5 O15 V2 129.0(4) 7_556 . . . ?
V4 V5 O15 V2 105.6(2) . . . . ?
V1 V5 O15 V2 24.8(3) . . . . ?
O21 V5 O15 V9 115.2(3) . . . 7_556 ?
O19 V5 O15 V9 -127.4(3) . . . 7_556 ?
O11 V5 O15 V9 -1.4(3) . . . 7_556 ?
O9 V5 O15 V9 -64.0(6) . . . 7_556 ?
V2 V5 O15 V9 -129.0(4) . . . 7_556 ?
V4 V5 O15 V9 -23.4(3) . . . 7_556 ?
V1 V5 O15 V9 -104.2(2) . . . 7_556 ?
O18 V2 O16 V8 156.7(4) . . . . ?
O19 V2 O16 V8 -33.4(10) . . . . ?
O14 V2 O16 V8 -98.9(4) . . . . ?
O15 V2 O16 V8 54.7(4) . . . . ?
V5 V2 O16 V8 34.2(5) . . . . ?
V7 V2 O16 V8 -98.1(4) . . . . ?
O18 V2 O16 V7 -105.3(4) . . . . ?
O19 V2 O16 V7 64.7(8) . . . . ?
O14 V2 O16 V7 -0.8(3) . . . . ?
O15 V2 O16 V7 152.8(3) . . . . ?
V5 V2 O16 V7 132.3(2) . . . . ?
O8 V8 O16 V2 -158.8(4) . . . . ?
O2 V8 O16 V2 29.8(10) . . . . ?
O23 V8 O16 V2 100.9(4) 7_556 . . . ?
O6 V8 O16 V2 -58.0(4) . . . . ?
O4 V8 O16 V2 12.2(3) . . . . ?
V10 V8 O16 V2 -36.5(5) . . . . ?
V7 V8 O16 V2 98.4(4) . . . . ?
O8 V8 O16 V7 102.8(3) . . . . ?
O2 V8 O16 V7 -68.5(8) . . . . ?
O23 V8 O16 V7 2.5(2) 7_556 . . . ?
O6 V8 O16 V7 -156.4(3) . . . . ?
O4 V8 O16 V7 -86.2(3) . . . . ?
V10 V8 O16 V7 -134.89(19) . . . . ?
O24 V7 O16 V2 118.6(4) . . . . ?
O14 V7 O16 V2 0.8(3) . . . . ?
O23 V7 O16 V2 -126.0(3) 7_556 . . . ?
O20 V7 O16 V2 -62.1(6) 7_556 . . . ?
V3 V7 O16 V2 -16.5(3) 7_556 . . . ?
V4 V7 O16 V2 -107.3(2) 7_556 . . . ?
V8 V7 O16 V2 -123.4(3) . . . . ?
O24 V7 O16 V8 -118.1(4) . . . . ?
O14 V7 O16 V8 124.2(3) . . . . ?
O23 V7 O16 V8 -2.6(3) 7_556 . . . ?
O20 V7 O16 V8 61.3(6) 7_556 . . . ?
V3 V7 O16 V8 106.8(2) 7_556 . . . ?
V4 V7 O16 V8 16.1(3) 7_556 . . . ?
V2 V7 O16 V8 123.4(3) . . . . ?
O21 V5 O19 V2 101.9(4) . . . . ?
O11 V5 O19 V2 -77.9(4) . . . . ?
O15 V5 O19 V2 -1.7(3) . . . . ?
O9 V5 O19 V2 -152.1(3) . . . . ?
V9 V5 O19 V2 -35.6(3) 7_556 . . . ?
V4 V5 O19 V2 -117.6(2) . . . . ?
V1 V5 O19 V2 -148.2(4) . . . . ?
O21 V5 O19 V1 -109.9(4) . . . . ?
O11 V5 O19 V1 70.3(4) . . . . ?
O15 V5 O19 V1 146.5(3) . . . . ?
O9 V5 O19 V1 -3.9(3) . . . . ?
V2 V5 O19 V1 148.2(4) . . . . ?
V9 V5 O19 V1 112.6(2) 7_556 . . . ?
V4 V5 O19 V1 30.6(3) . . . . ?
O18 V2 O19 V5 -97.6(4) . . . . ?
O14 V2 O19 V5 156.0(3) . . . . ?
O15 V2 O19 V5 1.7(3) . . . . ?
O16 V2 O19 V5 92.7(8) . . . . ?
V7 V2 O19 V5 140.89(18) . . . . ?
O18 V2 O19 V1 140.2(6) . . . . ?
O14 V2 O19 V1 33.9(6) . . . . ?
O15 V2 O19 V1 -120.4(6) . . . . ?
O16 V2 O19 V1 -29.5(11) . . . . ?
V5 V2 O19 V1 -122.2(7) . . . . ?
V7 V2 O19 V1 18.7(7) . . . . ?
O12 V1 O19 V5 94.1(4) . . . . ?
O13 V1 O19 V5 -159.5(3) . . . . ?
O10 V1 O19 V5 -87.4(8) . . . . ?
O9 V1 O19 V5 3.9(3) . . . . ?
O3 V1 O19 V5 -70.0(3) . . . . ?
O12 V1 O19 V2 -144.4(6) . . . . ?
O13 V1 O19 V2 -38.0(6) . . . . ?
O10 V1 O19 V2 34.1(11) . . . . ?
O9 V1 O19 V2 125.4(6) . . . . ?
O3 V1 O19 V2 51.5(6) . . . . ?
V5 V1 O19 V2 121.5(7) . . . . ?
O22 V3 O20 V4 -164.3(5) . . . . ?
O10 V3 O20 V4 -59.5(5) . . . . ?
O14 V3 O20 V4 92.3(5) 7_556 . . . ?
O13 V3 O20 V4 14.6(10) 7_556 . . . ?
V7 V3 O20 V4 95.8(5) 7_556 . . . ?
V6 V3 O20 V4 -40.8(6) . . . . ?
O22 V3 O20 V7 99.8(4) . . . 7_556 ?
O10 V3 O20 V7 -155.4(3) . . . 7_556 ?
O14 V3 O20 V7 -3.5(3) 7_556 . . 7_556 ?
O13 V3 O20 V7 -81.2(7) 7_556 . . 7_556 ?
V6 V3 O20 V7 -136.59(17) . . . 7_556 ?
O17 V4 O20 V3 166.3(5) . . . . ?
O23 V4 O20 V3 -93.6(4) . . . . ?
O11 V4 O20 V3 -16.7(10) . . . . ?
O9 V4 O20 V3 64.3(5) . . . . ?
O3 V4 O20 V3 -6.9(4) . . . . ?
V7 V4 O20 V3 -95.5(5) 7_556 . . . ?
V5 V4 O20 V3 41.9(6) . . . . ?
O17 V4 O20 V7 -98.2(3) . . . 7_556 ?
O23 V4 O20 V7 1.9(3) . . . 7_556 ?
O11 V4 O20 V7 78.9(8) . . . 7_556 ?
O9 V4 O20 V7 159.9(3) . . . 7_556 ?
O3 V4 O20 V7 88.6(3) . . . 7_556 ?
V5 V4 O20 V7 137.47(18) . . . 7_556 ?
O19 V5 O21 Mn1 -48.7(7) . . . 25_566 ?
O11 V5 O21 Mn1 131.1(6) . . . 25_566 ?
O15 V5 O21 Mn1 41.2(7) . . . 25_566 ?
O9 V5 O21 Mn1 -139.2(6) . . . 25_566 ?
V2 V5 O21 Mn1 -2.0(8) . . . 25_566 ?
V9 V5 O21 Mn1 84.5(7) 7_556 . . 25_566 ?
V4 V5 O21 Mn1 177.3(5) . . . 25_566 ?
V1 V5 O21 Mn1 -95.2(6) . . . 25_566 ?
O17 V4 O23 V7 98.5(3) . . . 7_556 ?
O11 V4 O23 V7 -160.1(3) . . . 7_556 ?
O20 V4 O23 V7 -2.0(3) . . . 7_556 ?
O9 V4 O23 V7 -94.7(7) . . . 7_556 ?
O3 V4 O23 V7 -75.7(3) . . . 7_556 ?
V5 V4 O23 V7 -143.35(15) . . . 7_556 ?
O17 V4 O23 V8 -132.6(6) . . . 7_556 ?
O11 V4 O23 V8 -31.2(6) . . . 7_556 ?
O20 V4 O23 V8 126.9(6) . . . 7_556 ?
O9 V4 O23 V8 34.2(11) . . . 7_556 ?
O3 V4 O23 V8 53.2(6) . . . 7_556 ?
V7 V4 O23 V8 128.9(7) 7_556 . . 7_556 ?
V5 V4 O23 V8 -14.4(7) . . . 7_556 ?
O14 V7 O24 Mn2 -44.7(11) . . . . ?
O23 V7 O24 Mn2 143.9(8) 7_556 . . . ?
O20 V7 O24 Mn2 50.1(10) 7_556 . . . ?
O16 V7 O24 Mn2 -130.3(9) . . . . ?
V3 V7 O24 Mn2 4.6(11) 7_556 . . . ?
V4 V7 O24 Mn2 95.5(9) 7_556 . . . ?
V8 V7 O24 Mn2 -173.2(7) . . . . ?
V2 V7 O24 Mn2 -87.8(9) . . . . ?
O24 Mn2 O24 V7 -96.0(10) 11_564 . . . ?
O28A Mn2 O24 V7 28.4(13) . . . . ?
O28A Mn2 O24 V7 139.7(12) 11_564 . . . ?
O28 Mn2 O24 V7 50.6(14) . . . . ?
O28 Mn2 O24 V7 117.4(14) 11_564 . . . ?
O27 Mn2 O24 V7 -51.3(10) . . . . ?
O27 Mn2 O24 V7 -140.5(10) 11_564 . . . ?

_diffrn_measured_fraction_theta_max 0.999
_diffrn_reflns_theta_full        25.08
_diffrn_measured_fraction_theta_full 0.999
_refine_diff_density_max         2.381
_refine_diff_density_min         -2.227
_refine_diff_density_rms         0.244
